# Supplementary Information (SI) for Journal of Materials Chemistry C.
# This journal is © The Royal Society of Chemistry 2024

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_222
_database_code_depnum_ccdc_archive 'CCDC 2371099'
loop_
_audit_author_name
_audit_author_address
'Haoran Wang'
;Xinjiang Technical Institute of Physics and Chemistry
China
;
_audit_update_record             
;
2024-07-16 deposited with the CCDC.	2024-08-12 downloaded from the CCDC.
;
_audit_creation_date             2021-08-15
_audit_creation_method           
;
Olex2 1.3
(compiled 2020.11.12 svn.r5f609507 for OlexSys, GUI svn.r6272)
;
_shelx_SHELXL_version_number     2016/6
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'Al2 B11 K3 O21'
_chemical_formula_sum            'Al2 B11 K3 O21'
_chemical_formula_weight         626.17
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Al Al 0.0645 0.0514 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
B B 0.0013 0.0007 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 1 21/c 1'
_space_group_name_Hall           '-P 2ybc'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'

_cell_length_a                   6.9336(8)
_cell_length_b                   22.240(3)
_cell_length_c                   13.3521(12)
_cell_angle_alpha                90
_cell_angle_beta                 117.994(5)
_cell_angle_gamma                90
_cell_volume                     1818.0(4)
_cell_formula_units_Z            4
_cell_measurement_reflns_used    1684
_cell_measurement_temperature    293.15
_cell_measurement_theta_max      27.30
_cell_measurement_theta_min      3.25
_shelx_estimated_absorpt_T_max   0.927
_shelx_estimated_absorpt_T_min   0.885
_exptl_absorpt_coefficient_mu    0.960
_exptl_absorpt_correction_T_max  0.7456
_exptl_absorpt_correction_T_min  0.5958
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
;
SADABS-2016/2 (Bruker,2016/2) was used for absorption correction.
wR2(int) was 0.0793 before and 0.0596 after correction.
The Ratio of minimum to maximum transmission is 0.7991.
The λ/2 correction factor is Not present.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            colourless
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    2.288
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       block
_exptl_crystal_F_000             1224
_exptl_crystal_size_max          0.13
_exptl_crystal_size_mid          0.087
_exptl_crystal_size_min          0.08
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0814
_diffrn_reflns_av_unetI/netI     0.0729
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.997
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       26
_diffrn_reflns_limit_k_min       -28
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            16212
_diffrn_reflns_point_group_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.530
_diffrn_reflns_theta_min         1.955
_diffrn_ambient_temperature      293.15
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_diffrn_source_current           1.4
_diffrn_source_power             0.07
_diffrn_source_voltage           50.0
_diffrn_standards_number         0
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                2603
_reflns_number_total             4166
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'SAINT V8.38A (Bruker, 2018)'
_computing_data_collection       ?
_computing_data_reduction        'SAINT V8.38A (Bruker, 2018)'
_computing_molecular_graphics    'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_structure_refinement  'XL  (Sheldrick, 2008)'
_computing_structure_solution    'SHELXT 2014/5 (Sheldrick, 2014)'
_refine_diff_density_max         0.672
_refine_diff_density_min         -0.582
_refine_diff_density_rms         0.103
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.975
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     334
_refine_ls_number_reflns         4166
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0882
_refine_ls_R_factor_gt           0.0488
_refine_ls_restrained_S_all      0.975
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0575P)²] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1086
_refine_ls_wR_factor_ref         0.1278
_refine_special_details          ?
_olex2_refinement_description    
;
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
K1 K 0.62186(14) -0.10695(4) 0.75188(8) 0.0332(2) Uani 1 1 d . . . . .
K2 K -0.38649(14) -0.07234(5) 0.25019(8) 0.0332(2) Uani 1 1 d . . . . .
K3 K -0.71605(16) -0.22819(5) 0.11580(9) 0.0428(3) Uani 1 1 d . . . . .
Al1 Al 0.09586(17) 0.09241(5) 0.90791(9) 0.0185(3) Uani 1 1 d . . . . .
Al2 Al -0.08793(17) -0.09192(5) 0.58685(10) 0.0201(3) Uani 1 1 d . . . . .
B1 B 0.1876(7) -0.08138(19) 0.9977(4) 0.0207(9) Uani 1 1 d . . . . .
B2 B 0.4704(6) -0.06569(19) 0.9435(3) 0.0178(8) Uani 1 1 d . . . . .
B3 B 0.0997(6) -0.03308(19) 0.8180(4) 0.0193(9) Uani 1 1 d . . . . .
B4 B -0.1141(6) 0.02537(19) 0.6855(4) 0.0195(9) Uani 1 1 d . . . . .
B5 B -0.4821(6) 0.05996(19) 0.5593(4) 0.0203(9) Uani 1 1 d . . . . .
B6 B -0.2003(6) 0.07365(19) 0.5036(4) 0.0202(9) Uani 1 1 d . . . . .
B7 B -0.2356(7) -0.2027(2) 0.5307(4) 0.0242(10) Uani 1 1 d . . . . .
B8 B -0.5082(7) -0.2725(2) 0.4108(4) 0.0245(10) Uani 1 1 d . . . . .
B9 B -0.2140(7) -0.24709(19) 0.3637(4) 0.0218(9) Uani 1 1 d . . . . .
B10 B -0.1203(7) -0.19484(19) 0.2280(4) 0.0234(9) Uani 1 1 d . . . . .
B11 B 0.1036(7) -0.2751(2) 0.3415(4) 0.0232(9) Uani 1 1 d . . . . .
O1 O 0.1364(4) -0.10232(12) 1.0768(2) 0.0230(6) Uani 1 1 d . . . . .
O2 O 0.4074(4) -0.07968(12) 1.0249(2) 0.0233(6) Uani 1 1 d . . . . .
O3 O 0.6799(4) -0.07152(12) 0.9667(2) 0.0229(6) Uani 1 1 d . . . . .
O4 O 0.0366(4) -0.06092(12) 0.8944(2) 0.0228(6) Uani 1 1 d . . . . .
O5 O 0.3182(4) -0.04467(11) 0.8395(2) 0.0220(6) Uani 1 1 d . . . . .
O6 O 0.0503(4) 0.03468(11) 0.8069(2) 0.0209(6) Uani 1 1 d . . . . .
O7 O -0.0663(4) -0.04292(11) 0.6965(2) 0.0200(6) Uani 1 1 d . . . . .
O8 O -0.3322(4) 0.03837(11) 0.6628(2) 0.0216(6) Uani 1 1 d . . . . .
O9 O -0.0508(4) 0.05273(12) 0.6088(2) 0.0231(6) Uani 1 1 d . . . . .
O10 O -0.6927(4) 0.06477(12) 0.5357(2) 0.0248(6) Uani 1 1 d . . . . .
O11 O -0.4184(4) 0.07641(12) 0.4797(2) 0.0264(6) Uani 1 1 d . . . . .
O12 O -0.1505(4) 0.09102(12) 0.4239(2) 0.0254(6) Uani 1 1 d . . . . .
O13 O -0.1629(4) -0.16183(12) 0.6148(2) 0.0266(6) Uani 1 1 d . . . . .
O14 O -0.4283(4) -0.23464(12) 0.5018(2) 0.0293(6) Uani 1 1 d . . . . .
O15 O -0.1275(4) -0.21278(13) 0.4696(2) 0.0294(6) Uani 1 1 d . . . . .
O16 O -0.4149(4) -0.27940(12) 0.3429(2) 0.0265(6) Uani 1 1 d . . . . .
O17 O -0.2653(4) -0.20567(12) 0.2682(2) 0.0253(6) Uani 1 1 d . . . . .
O18 O -0.0455(4) -0.29096(12) 0.3746(2) 0.0257(6) Uani 1 1 d . . . . .
O19 O -0.1560(4) -0.15307(12) 0.1496(2) 0.0291(6) Uani 1 1 d . . . . .
O20 O 0.0730(4) -0.22789(12) 0.2695(2) 0.0281(6) Uani 1 1 d . . . . .
O21 O 0.3018(4) -0.30376(12) 0.3882(2) 0.0289(7) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
K1 B2 3.319(4) . ?
K1 B3 3.422(4) 1_655 ?
K1 B6 3.372(4) 3_556 ?
K1 O3 2.816(3) . ?
K1 O4 2.793(3) 1_655 ?
K1 O5 3.167(3) . ?
K1 O7 2.958(3) 1_655 ?
K1 O11 2.814(3) 3_556 ?
K1 O12 3.019(3) 3_556 ?
K1 O13 3.104(3) 1_655 ?
K1 O16 2.867(3) 4_656 ?
K1 O18 3.100(3) 4_656 ?
K2 B1 3.284(4) 1_454 ?
K2 B4 3.328(4) 3_556 ?
K2 B5 3.091(5) 3_456 ?
K2 O1 3.092(3) 1_454 ?
K2 O2 2.661(3) 1_454 ?
K2 O5 2.994(3) 3_556 ?
K2 O6 2.896(3) 3_556 ?
K2 O8 2.802(3) 3_456 ?
K2 O9 2.751(2) 3_556 ?
K2 O10 2.651(3) 3_456 ?
K2 O17 3.060(3) . ?
K2 O19 3.098(3) . ?
K3 B1 3.551(4) 1_454 ?
K3 B9 3.526(4) . ?
K3 B9 3.556(4) 4_455 ?
K3 B11 3.269(5) 4_455 ?
K3 O1 2.942(3) 1_454 ?
K3 O14 3.136(3) 4 ?
K3 O15 2.906(3) 4_455 ?
K3 O16 2.985(3) . ?
K3 O17 2.862(3) . ?
K3 O18 2.978(3) 4_455 ?
K3 O20 3.028(3) 1_455 ?
K3 O21 3.179(3) 4_455 ?
Al1 O1 1.730(3) 3_557 ?
Al1 O3 1.730(3) 3_657 ?
Al1 O6 1.780(3) . ?
Al1 O19 1.698(3) 3_556 ?
Al2 O7 1.774(3) . ?
Al2 O10 1.738(3) 3_456 ?
Al2 O12 1.725(3) 3_556 ?
Al2 O13 1.734(3) . ?
B1 O1 1.346(5) . ?
B1 O2 1.391(5) . ?
B1 O4 1.359(5) . ?
B2 O2 1.384(5) . ?
B2 O3 1.342(4) . ?
B2 O5 1.372(4) . ?
B3 B4 2.135(6) . ?
B3 O4 1.427(5) . ?
B3 O5 1.427(5) . ?
B3 O6 1.537(5) . ?
B3 O7 1.501(5) . ?
B4 O6 1.495(5) . ?
B4 O7 1.547(5) . ?
B4 O8 1.425(4) . ?
B4 O9 1.426(5) . ?
B5 O8 1.369(5) . ?
B5 O10 1.346(5) . ?
B5 O11 1.378(5) . ?
B6 O9 1.377(5) . ?
B6 O11 1.393(5) . ?
B6 O12 1.322(5) . ?
B7 O13 1.346(5) . ?
B7 O14 1.398(5) . ?
B7 O15 1.360(5) . ?
B8 O14 1.364(5) . ?
B8 O16 1.346(5) . ?
B8 O21 1.392(5) 1_455 ?
B9 O15 1.465(5) . ?
B9 O16 1.473(5) . ?
B9 O17 1.474(5) . ?
B9 O18 1.476(5) . ?
B10 O17 1.366(5) . ?
B10 O19 1.333(5) . ?
B10 O20 1.395(5) . ?
B11 O18 1.349(5) . ?
B11 O20 1.370(5) . ?
B11 O21 1.371(5) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
B2 K1 B3 106.66(10) . 1_655 ?
B2 K1 B6 106.34(10) . 3_556 ?
B6 K1 B3 115.48(11) 3_556 1_655 ?
O3 K1 B2 23.48(8) . . ?
O3 K1 B3 86.83(9) . 1_655 ?
O3 K1 B6 127.64(10) . 3_556 ?
O3 K1 O5 45.83(6) . . ?
O3 K1 O7 110.38(8) . 1_655 ?
O3 K1 O12 110.11(8) . 3_556 ?
O3 K1 O13 146.37(7) . 1_655 ?
O3 K1 O16 79.24(8) . 4_656 ?
O3 K1 O18 87.21(7) . 4_656 ?
O4 K1 B2 88.30(9) 1_655 . ?
O4 K1 B3 23.91(9) 1_655 1_655 ?
O4 K1 B6 137.33(10) 1_655 3_556 ?
O4 K1 O3 66.05(8) 1_655 . ?
O4 K1 O5 103.78(8) 1_655 . ?
O4 K1 O7 49.80(7) 1_655 1_655 ?
O4 K1 O11 119.03(8) 1_655 3_556 ?
O4 K1 O12 151.56(8) 1_655 3_556 ?
O4 K1 O13 85.40(8) 1_655 1_655 ?
O4 K1 O16 107.59(8) 1_655 4_656 ?
O4 K1 O18 68.64(7) 1_655 4_656 ?
O5 K1 B2 24.29(8) . . ?
O5 K1 B3 115.19(9) . 1_655 ?
O5 K1 B6 82.35(9) . 3_556 ?
O7 K1 B2 126.34(9) 1_655 . ?
O7 K1 B3 25.93(8) 1_655 1_655 ?
O7 K1 B6 91.69(9) 1_655 3_556 ?
O7 K1 O5 124.92(7) 1_655 . ?
O7 K1 O12 113.63(7) 1_655 3_556 ?
O7 K1 O13 55.36(7) 1_655 1_655 ?
O7 K1 O18 92.01(7) 1_655 4_656 ?
O11 K1 B2 127.12(9) 3_556 . ?
O11 K1 B3 95.34(9) 3_556 1_655 ?
O11 K1 B6 23.90(9) 3_556 3_556 ?
O11 K1 O3 144.11(8) 3_556 . ?
O11 K1 O5 102.88(7) 3_556 . ?
O11 K1 O7 69.96(7) 3_556 1_655 ?
O11 K1 O12 46.85(8) 3_556 3_556 ?
O11 K1 O13 65.08(7) 3_556 1_655 ?
O11 K1 O16 125.46(8) 3_556 4_656 ?
O11 K1 O18 128.50(8) 3_556 4_656 ?
O12 K1 B2 87.01(9) 3_556 . ?
O12 K1 B3 135.08(9) 3_556 1_655 ?
O12 K1 B6 23.03(9) 3_556 3_556 ?
O12 K1 O5 64.60(7) 3_556 . ?
O12 K1 O13 103.45(8) 3_556 1_655 ?
O12 K1 O18 139.65(8) 3_556 4_656 ?
O13 K1 B2 167.76(9) 1_655 . ?
O13 K1 B3 70.47(9) 1_655 1_655 ?
O13 K1 B6 85.30(9) 1_655 3_556 ?
O13 K1 O5 167.65(7) 1_655 . ?
O16 K1 B2 78.09(9) 4_656 . ?
O16 K1 B3 125.58(9) 4_656 1_655 ?
O16 K1 B6 114.53(9) 4_656 3_556 ?
O16 K1 O5 91.26(8) 4_656 . ?
O16 K1 O7 138.70(8) 4_656 1_655 ?
O16 K1 O12 98.84(8) 4_656 3_556 ?
O16 K1 O13 93.82(8) 4_656 1_655 ?
O16 K1 O18 47.36(7) 4_656 4_656 ?
O18 K1 B2 102.78(9) 4_656 . ?
O18 K1 B3 79.93(9) 4_656 1_655 ?
O18 K1 B6 140.55(9) 4_656 3_556 ?
O18 K1 O5 125.70(8) 4_656 . ?
O18 K1 O13 65.13(7) 4_656 1_655 ?
B1 K2 B4 127.61(11) 1_454 3_556 ?
B5 K2 B1 112.34(11) 3_456 1_454 ?
B5 K2 B4 115.75(11) 3_456 3_556 ?
B5 K2 O1 90.60(9) 3_456 1_454 ?
B5 K2 O19 145.08(10) 3_456 . ?
O1 K2 B1 24.13(9) 1_454 1_454 ?
O1 K2 B4 151.71(10) 1_454 3_556 ?
O1 K2 O19 97.98(7) 1_454 . ?
O2 K2 B1 24.30(10) 1_454 1_454 ?
O2 K2 B4 104.63(10) 1_454 3_556 ?
O2 K2 B5 136.59(10) 1_454 3_456 ?
O2 K2 O1 47.32(8) 1_454 1_454 ?
O2 K2 O5 72.72(8) 1_454 3_556 ?
O2 K2 O6 77.98(8) 1_454 3_556 ?
O2 K2 O8 112.09(8) 1_454 3_456 ?
O2 K2 O9 128.16(9) 1_454 3_556 ?
O2 K2 O17 90.66(8) 1_454 . ?
O2 K2 O19 65.60(8) 1_454 . ?
O5 K2 B1 82.95(9) 3_556 1_454 ?
O5 K2 B4 59.26(8) 3_556 3_556 ?
O5 K2 B5 114.51(10) 3_556 3_456 ?
O5 K2 O1 101.67(7) 3_556 1_454 ?
O5 K2 O17 141.68(8) 3_556 . ?
O5 K2 O19 96.87(8) 3_556 . ?
O6 K2 B1 101.22(10) 3_556 1_454 ?
O6 K2 B4 26.64(9) 3_556 3_556 ?
O6 K2 B5 140.86(10) 3_556 3_456 ?
O6 K2 O1 125.16(8) 3_556 1_454 ?
O6 K2 O5 49.10(7) 3_556 3_556 ?
O6 K2 O17 94.35(7) 3_556 . ?
O6 K2 O19 53.89(7) 3_556 . ?
O8 K2 B1 88.66(10) 3_456 1_454 ?
O8 K2 B4 130.77(10) 3_456 3_556 ?
O8 K2 B5 26.28(9) 3_456 3_456 ?
O8 K2 O1 70.14(7) 3_456 1_454 ?
O8 K2 O5 101.71(8) 3_456 3_556 ?
O8 K2 O6 146.53(8) 3_456 3_556 ?
O8 K2 O17 116.58(8) 3_456 . ?
O8 K2 O19 159.58(8) 3_456 . ?
O9 K2 B1 152.06(10) 3_556 1_454 ?
O9 K2 B4 24.89(9) 3_556 3_556 ?
O9 K2 B5 94.51(10) 3_556 3_456 ?
O9 K2 O1 174.16(8) 3_556 1_454 ?
O9 K2 O5 78.79(7) 3_556 3_556 ?
O9 K2 O6 50.91(7) 3_556 3_556 ?
O9 K2 O8 115.57(8) 3_556 3_456 ?
O9 K2 O17 85.76(8) 3_556 . ?
O9 K2 O19 76.20(8) 3_556 . ?
O10 K2 B1 137.93(10) 3_456 1_454 ?
O10 K2 B4 92.23(10) 3_456 3_556 ?
O10 K2 B5 25.67(9) 3_456 3_456 ?
O10 K2 O1 115.37(8) 3_456 1_454 ?
O10 K2 O2 162.23(9) 3_456 1_454 ?
O10 K2 O5 112.62(8) 3_456 3_556 ?
O10 K2 O6 118.72(8) 3_456 3_556 ?
O10 K2 O8 50.81(7) 3_456 3_456 ?
O10 K2 O9 69.40(8) 3_456 3_556 ?
O10 K2 O17 93.81(8) 3_456 . ?
O10 K2 O19 128.06(8) 3_456 . ?
O17 K2 B1 95.90(9) . 1_454 ?
O17 K2 B4 93.97(9) . 3_556 ?
O17 K2 B5 101.40(10) . 3_456 ?
O17 K2 O1 90.45(7) . 1_454 ?
O17 K2 O19 45.11(7) . . ?
O19 K2 B1 85.27(9) . 1_454 ?
O19 K2 B4 66.79(9) . 3_556 ?
B1 K3 B9 79.92(10) 1_454 4_455 ?
B9 K3 B1 115.06(10) . 1_454 ?
B9 K3 B9 164.22(4) . 4_455 ?
B11 K3 B1 65.70(11) 4_455 1_454 ?
B11 K3 B9 41.57(11) 4_455 4_455 ?
B11 K3 B9 138.11(11) 4_455 . ?
O1 K3 B1 21.40(9) 1_454 1_454 ?
O1 K3 B9 112.82(9) 1_454 . ?
O1 K3 B9 82.93(9) 1_454 4_455 ?
O1 K3 B11 82.07(10) 1_454 4_455 ?
O1 K3 O14 114.36(8) 1_454 4 ?
O1 K3 O16 124.22(8) 1_454 . ?
O1 K3 O18 69.25(7) 1_454 4_455 ?
O1 K3 O20 83.07(8) 1_454 1_455 ?
O1 K3 O21 77.54(8) 1_454 4_455 ?
O14 K3 B1 93.24(9) 4 1_454 ?
O14 K3 B9 93.21(9) 4 4_455 ?
O14 K3 B9 81.47(9) 4 . ?
O14 K3 B11 57.16(9) 4 4_455 ?
O14 K3 O21 43.59(7) 4 4_455 ?
O15 K3 B1 101.32(9) 4_455 1_454 ?
O15 K3 B9 23.56(9) 4_455 4_455 ?
O15 K3 B9 143.33(10) 4_455 . ?
O15 K3 B11 61.23(10) 4_455 4_455 ?
O15 K3 O1 99.24(8) 4_455 1_454 ?
O15 K3 O14 101.68(8) 4_455 4 ?
O15 K3 O16 120.54(8) 4_455 . ?
O15 K3 O18 47.56(8) 4_455 4_455 ?
O15 K3 O20 79.75(8) 4_455 1_455 ?
O15 K3 O21 85.72(8) 4_455 4_455 ?
O16 K3 B1 134.29(9) . 1_454 ?
O16 K3 B9 143.92(9) . 4_455 ?
O16 K3 B9 24.39(9) . . ?
O16 K3 B11 149.79(10) . 4_455 ?
O16 K3 O14 95.26(8) . 4 ?
O16 K3 O20 69.05(8) . 1_455 ?
O16 K3 O21 137.21(8) . 4_455 ?
O17 K3 B1 94.01(9) . 1_454 ?
O17 K3 B9 162.06(10) . 4_455 ?
O17 K3 B9 23.91(9) . . ?
O17 K3 B11 120.59(10) . 4_455 ?
O17 K3 O1 97.61(8) . 1_454 ?
O17 K3 O14 70.14(8) . 4 ?
O17 K3 O15 163.12(9) . 4_455 ?
O17 K3 O16 48.28(7) . . ?
O17 K3 O18 140.50(9) . 4_455 ?
O17 K3 O20 103.37(8) . 1_455 ?
O17 K3 O21 96.96(8) . 4_455 ?
O18 K3 B1 59.93(8) 4_455 1_454 ?
O18 K3 B9 24.09(9) 4_455 4_455 ?
O18 K3 B9 161.91(10) 4_455 . ?
O18 K3 B11 24.37(9) 4_455 4_455 ?
O18 K3 O14 81.52(8) 4_455 4 ?
O18 K3 O16 165.75(8) 4_455 . ?
O18 K3 O20 111.30(8) 4_455 1_455 ?
O18 K3 O21 44.64(7) 4_455 4_455 ?
O20 K3 B1 104.42(9) 1_455 1_454 ?
O20 K3 B9 94.50(9) 1_455 4_455 ?
O20 K3 B9 86.69(9) 1_455 . ?
O20 K3 B11 134.98(10) 1_455 4_455 ?
O20 K3 O14 161.71(8) 1_455 4 ?
O20 K3 O21 153.53(7) 1_455 4_455 ?
O21 K3 B1 56.86(9) 4_455 1_454 ?
O21 K3 B9 65.54(9) 4_455 4_455 ?
O21 K3 B9 117.37(9) 4_455 . ?
O21 K3 B11 24.51(9) 4_455 4_455 ?
K2 Al1 K3 126.41(4) 3_556 3_456 ?
O1 Al1 K2 154.45(10) 3_557 3_556 ?
O1 Al1 K3 44.30(9) 3_557 3_456 ?
O1 Al1 O6 109.73(13) 3_557 . ?
O3 Al1 K2 92.19(10) 3_657 3_556 ?
O3 Al1 K3 123.34(10) 3_657 3_456 ?
O3 Al1 O1 112.55(14) 3_657 3_557 ?
O3 Al1 O6 107.39(13) 3_657 . ?
O6 Al1 K2 53.81(9) . 3_556 ?
O6 Al1 K3 128.38(9) . 3_456 ?
O19 Al1 K2 60.32(11) 3_556 3_556 ?
O19 Al1 K3 69.49(10) 3_556 3_456 ?
O19 Al1 O1 113.08(14) 3_556 3_557 ?
O19 Al1 O3 110.55(14) 3_556 3_657 ?
O19 Al1 O6 102.97(14) 3_556 . ?
K1 Al2 K2 123.45(3) 1_455 . ?
O7 Al2 K1 53.97(9) . 1_455 ?
O7 Al2 K2 131.32(9) . . ?
O10 Al2 K1 96.54(10) 3_456 1_455 ?
O10 Al2 K2 30.68(9) 3_456 . ?
O10 Al2 O7 105.13(13) 3_456 . ?
O12 Al2 K1 151.31(10) 3_556 1_455 ?
O12 Al2 K2 85.18(9) 3_556 . ?
O12 Al2 O7 110.38(13) 3_556 . ?
O12 Al2 O10 111.55(14) 3_556 3_456 ?
O12 Al2 O13 115.08(14) 3_556 . ?
O13 Al2 K1 58.64(10) . 1_455 ?
O13 Al2 K2 106.88(9) . . ?
O13 Al2 O7 106.92(14) . . ?
O13 Al2 O10 107.20(13) . 3_456 ?
K2 B1 K3 73.09(8) 1_656 1_656 ?
O1 B1 K2 69.93(19) . 1_656 ?
O1 B1 K3 52.92(19) . 1_656 ?
O1 B1 O2 117.7(3) . . ?
O1 B1 O4 123.4(4) . . ?
O2 B1 K2 51.91(18) . 1_656 ?
O2 B1 K3 87.4(2) . 1_656 ?
O4 B1 K2 156.1(3) . 1_656 ?
O4 B1 K3 130.8(3) . 1_656 ?
O4 B1 O2 119.0(4) . . ?
O2 B2 K1 150.9(3) . . ?
O3 B2 K1 56.74(19) . . ?
O3 B2 O2 120.2(3) . . ?
O3 B2 O5 120.1(4) . . ?
O5 B2 K1 71.7(2) . . ?
O5 B2 O2 119.7(3) . . ?
K1 B3 K2 149.71(13) 1_455 3_556 ?
B4 B3 K1 82.35(16) . 1_455 ?
B4 B3 K2 68.32(16) . 3_556 ?
O4 B3 K1 52.50(16) . 1_455 ?
O4 B3 K2 152.8(3) . 3_556 ?
O4 B3 B4 122.0(3) . . ?
O4 B3 O6 111.4(3) . . ?
O4 B3 O7 111.9(3) . . ?
O5 B3 K1 140.6(2) . 1_455 ?
O5 B3 K2 59.24(18) . 3_556 ?
O5 B3 B4 122.4(3) . . ?
O5 B3 O4 115.5(3) . . ?
O5 B3 O6 111.4(3) . . ?
O5 B3 O7 113.2(3) . . ?
O6 B3 K1 107.5(2) . 1_455 ?
O6 B3 K2 55.94(17) . 3_556 ?
O6 B3 B4 44.44(18) . . ?
O7 B3 K1 59.50(17) . 1_455 ?
O7 B3 K2 93.3(2) . 3_556 ?
O7 B3 B4 46.43(18) . . ?
O7 B3 O6 90.9(2) . . ?
B3 B4 K2 75.10(15) . 3_556 ?
O6 B4 K2 60.32(17) . 3_556 ?
O6 B4 B3 46.06(18) . . ?
O6 B4 O7 90.7(2) . . ?
O7 B4 K2 97.63(19) . 3_556 ?
O7 B4 B3 44.67(17) . . ?
O8 B4 K2 149.9(3) . 3_556 ?
O8 B4 B3 123.7(3) . . ?
O8 B4 O6 113.3(3) . . ?
O8 B4 O7 112.2(3) . . ?
O8 B4 O9 114.5(3) . . ?
O9 B4 K2 54.27(16) . 3_556 ?
O9 B4 B3 121.8(3) . . ?
O9 B4 O6 112.6(3) . . ?
O9 B4 O7 111.3(3) . . ?
O8 B5 K2 65.0(2) . 3_456 ?
O8 B5 O11 120.4(3) . . ?
O10 B5 K2 58.6(2) . 3_456 ?
O10 B5 O8 119.4(4) . . ?
O10 B5 O11 120.2(3) . . ?
O11 B5 K2 159.4(3) . 3_456 ?
O9 B6 K1 170.4(3) . 3_556 ?
O9 B6 O11 117.7(4) . . ?
O11 B6 K1 54.96(18) . 3_556 ?
O12 B6 K1 63.33(19) . 3_556 ?
O12 B6 O9 124.3(4) . . ?
O12 B6 O11 117.9(3) . . ?
O13 B7 K3 95.7(2) . 4_656 ?
O13 B7 O14 120.6(4) . . ?
O13 B7 O15 121.0(4) . . ?
O14 B7 K3 124.0(3) . 4_656 ?
O15 B7 K3 50.49(19) . 4_656 ?
O15 B7 O14 118.4(4) . . ?
O14 B8 O21 116.7(4) . 1_455 ?
O16 B8 O14 123.2(4) . . ?
O16 B8 O21 120.2(4) . 1_455 ?
K1 B9 K3 103.60(11) 4_455 4_656 ?
K3 B9 K1 74.48(9) . 4_455 ?
K3 B9 K3 177.64(14) . 4_656 ?
O15 B9 K1 142.4(3) . 4_455 ?
O15 B9 K3 52.48(17) . 4_656 ?
O15 B9 K3 128.4(2) . . ?
O15 B9 O16 111.0(3) . . ?
O15 B9 O17 109.4(3) . . ?
O15 B9 O18 107.6(3) . . ?
O16 B9 K1 51.94(18) . 4_455 ?
O16 B9 K3 121.0(2) . 4_656 ?
O16 B9 K3 56.76(17) . . ?
O16 B9 O17 108.6(3) . . ?
O16 B9 O18 109.3(3) . . ?
O17 B9 K1 108.1(2) . 4_455 ?
O17 B9 K3 130.4(2) . 4_656 ?
O17 B9 K3 51.89(16) . . ?
O17 B9 O18 110.9(3) . . ?
O18 B9 K1 61.12(18) . 4_455 ?
O18 B9 K3 55.43(17) . 4_656 ?
O18 B9 K3 123.9(2) . . ?
O17 B10 K2 64.8(2) . . ?
O17 B10 O20 119.9(4) . . ?
O19 B10 K2 66.4(2) . . ?
O19 B10 O17 122.2(4) . . ?
O19 B10 O20 117.9(4) . . ?
O20 B10 K2 148.4(3) . . ?
O18 B11 K3 65.6(2) . 4_656 ?
O18 B11 O20 122.7(3) . . ?
O18 B11 O21 119.2(4) . . ?
O20 B11 K3 128.4(3) . 4_656 ?
O20 B11 O21 117.9(4) . . ?
O21 B11 K3 74.1(2) . 4_656 ?
K3 O1 K2 84.92(7) 1_656 1_656 ?
Al1 O1 K2 127.74(13) 3_557 1_656 ?
Al1 O1 K3 111.46(12) 3_557 1_656 ?
B1 O1 K2 85.9(2) . 1_656 ?
B1 O1 K3 105.7(2) . 1_656 ?
B1 O1 Al1 130.7(2) . 3_557 ?
B1 O2 K2 103.8(2) . 1_656 ?
B2 O2 K2 132.4(2) . 1_656 ?
B2 O2 B1 120.7(3) . . ?
Al1 O3 K1 122.99(13) 3_657 . ?
B2 O3 K1 99.8(2) . . ?
B2 O3 Al1 129.3(3) . 3_657 ?
B1 O4 K1 128.7(2) . 1_455 ?
B1 O4 B3 121.4(3) . . ?
B3 O4 K1 103.6(2) . 1_455 ?
K2 O5 K1 88.57(7) 3_556 . ?
B2 O5 K1 84.0(2) . . ?
B2 O5 K2 120.7(2) . 3_556 ?
B2 O5 B3 120.3(3) . . ?
B3 O5 K1 146.3(2) . . ?
B3 O5 K2 96.6(2) . 3_556 ?
Al1 O6 K2 96.44(11) . 3_556 ?
B3 O6 K2 98.0(2) . 3_556 ?
B3 O6 Al1 133.0(2) . . ?
B4 O6 K2 93.0(2) . 3_556 ?
B4 O6 Al1 134.1(2) . . ?
B4 O6 B3 89.5(3) . . ?
Al2 O7 K1 97.01(10) . 1_455 ?
B3 O7 K1 94.6(2) . 1_455 ?
B3 O7 Al2 134.9(2) . . ?
B3 O7 B4 88.9(3) . . ?
B4 O7 K1 110.3(2) . 1_455 ?
B4 O7 Al2 126.4(2) . . ?
B4 O8 K2 147.4(2) . 3_456 ?
B5 O8 K2 88.7(2) . 3_456 ?
B5 O8 B4 120.8(3) . . ?
B4 O9 K2 100.84(19) . 3_556 ?
B6 O9 K2 134.8(2) . 3_556 ?
B6 O9 B4 122.6(3) . . ?
Al2 O10 K2 129.78(14) 3_456 3_456 ?
B5 O10 K2 95.7(2) . 3_456 ?
B5 O10 Al2 128.5(3) . 3_456 ?
B5 O11 K1 137.3(2) . 3_556 ?
B5 O11 B6 121.2(3) . . ?
B6 O11 K1 101.1(2) . 3_556 ?
Al2 O12 K1 131.62(13) 3_556 3_556 ?
B6 O12 K1 93.6(2) . 3_556 ?
B6 O12 Al2 133.9(2) . 3_556 ?
Al2 O13 K1 92.86(11) . 1_455 ?
B7 O13 K1 131.5(2) . 1_455 ?
B7 O13 Al2 117.3(3) . . ?
B7 O14 K3 138.0(3) . 4_556 ?
B8 O14 K3 100.6(2) . 4_556 ?
B8 O14 B7 119.7(4) . . ?
B7 O15 K3 108.3(2) . 4_656 ?
B7 O15 B9 125.0(3) . . ?
B9 O15 K3 104.0(2) . 4_656 ?
K1 O16 K3 93.70(8) 4_455 . ?
B8 O16 K1 123.5(3) . 4_455 ?
B8 O16 K3 108.2(2) . . ?
B8 O16 B9 121.9(3) . . ?
B9 O16 K1 104.2(2) . 4_455 ?
B9 O16 K3 98.8(2) . . ?
K3 O17 K2 86.90(7) . . ?
B9 O17 K2 128.3(2) . . ?
B9 O17 K3 104.2(2) . . ?
B10 O17 K2 91.4(2) . . ?
B10 O17 K3 120.7(2) . . ?
B10 O17 B9 121.8(3) . . ?
K3 O18 K1 132.78(9) 4_656 4_455 ?
B9 O18 K1 94.2(2) . 4_455 ?
B9 O18 K3 100.5(2) . 4_656 ?
B11 O18 K1 120.9(3) . 4_455 ?
B11 O18 K3 90.0(2) . 4_656 ?
B11 O18 B9 119.2(3) . . ?
Al1 O19 K2 91.24(12) 3_556 . ?
B10 O19 K2 90.4(2) . . ?
B10 O19 Al1 156.1(3) . 3_556 ?
B10 O20 K3 114.3(2) . 1_655 ?
B11 O20 K3 120.6(2) . 1_655 ?
B11 O20 B10 119.0(3) . . ?
B8 O21 K3 98.0(2) 1_655 4_656 ?
B11 O21 K3 81.4(2) . 4_656 ?
B11 O21 B8 120.7(3) . 1_655 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
K1 Al2 O7 B3 103.7(3) 1_455 . . . ?
K1 Al2 O7 B4 -121.7(3) 1_455 . . . ?
K1 Al2 O13 B7 140.6(3) 1_455 . . . ?
K1 B2 O2 K2 106.6(5) . . . 1_656 ?
K1 B2 O2 B1 -96.6(5) . . . . ?
K1 B2 O3 Al1 -148.8(3) . . . 3_657 ?
K1 B2 O5 K2 -84.77(17) . . . 3_556 ?
K1 B2 O5 B3 155.2(3) . . . . ?
K1 B3 O4 B1 154.3(4) 1_455 . . . ?
K1 B3 O5 K1 51.8(6) 1_455 . . . ?
K1 B3 O5 K2 149.2(3) 1_455 . . 3_556 ?
K1 B3 O5 B2 -79.4(5) 1_455 . . . ?
K1 B3 O6 K2 -151.61(12) 1_455 . . 3_556 ?
K1 B3 O6 Al1 101.8(3) 1_455 . . . ?
K1 B3 O6 B4 -58.6(2) 1_455 . . . ?
K1 B3 O7 Al2 -104.6(3) 1_455 . . . ?
K1 B3 O7 B4 110.3(2) 1_455 . . . ?
K1 B6 O11 B5 174.0(4) 3_556 . . . ?
K1 B6 O12 Al2 -169.9(4) 3_556 . . 3_556 ?
K1 B9 O15 K3 59.3(4) 4_455 . . 4_656 ?
K1 B9 O15 B7 -65.4(6) 4_455 . . . ?
K1 B9 O16 K3 -96.13(13) 4_455 . . . ?
K1 B9 O16 B8 145.9(4) 4_455 . . . ?
K1 B9 O17 K2 149.55(13) 4_455 . . . ?
K1 B9 O17 K3 52.17(19) 4_455 . . . ?
K1 B9 O17 B10 -88.8(3) 4_455 . . . ?
K1 B9 O18 K3 -134.94(13) 4_455 . . 4_656 ?
K1 B9 O18 B11 129.1(3) 4_455 . . . ?
K2 Al1 O6 B3 107.2(3) 3_556 . . . ?
K2 Al1 O6 B4 -100.6(3) 3_556 . . . ?
K2 Al2 O7 K1 105.55(10) . . . 1_455 ?
K2 Al2 O7 B3 -150.8(3) . . . . ?
K2 Al2 O7 B4 -16.2(3) . . . . ?
K2 Al2 O13 K1 -119.31(6) . . . 1_455 ?
K2 Al2 O13 B7 21.3(3) . . . . ?
K2 B1 O1 K3 -83.57(10) 1_656 . . 1_656 ?
K2 B1 O1 Al1 138.5(3) 1_656 . . 3_557 ?
K2 B1 O2 B2 -162.5(4) 1_656 . . . ?
K2 B1 O4 K1 -157.7(5) 1_656 . . 1_455 ?
K2 B1 O4 B3 55.0(8) 1_656 . . . ?
K2 B3 O4 K1 152.6(4) 3_556 . . 1_455 ?
K2 B3 O4 B1 -53.1(7) 3_556 . . . ?
K2 B3 O5 K1 -97.3(4) 3_556 . . . ?
K2 B3 O5 B2 131.5(3) 3_556 . . . ?
K2 B3 O6 Al1 -106.6(3) 3_556 . . . ?
K2 B3 O6 B4 93.0(2) 3_556 . . . ?
K2 B3 O7 K1 -165.82(9) 3_556 . . 1_455 ?
K2 B3 O7 Al2 89.5(3) 3_556 . . . ?
K2 B3 O7 B4 -55.5(2) 3_556 . . . ?
K2 B4 O6 Al1 102.0(3) 3_556 . . . ?
K2 B4 O6 B3 -98.0(2) 3_556 . . . ?
K2 B4 O7 K1 154.17(9) 3_556 . . 1_455 ?
K2 B4 O7 Al2 -90.1(2) 3_556 . . . ?
K2 B4 O7 B3 59.7(2) 3_556 . . . ?
K2 B4 O8 K2 -73.8(7) 3_556 . . 3_456 ?
K2 B4 O8 B5 78.3(6) 3_556 . . . ?
K2 B4 O9 B6 -166.8(4) 3_556 . . . ?
K2 B5 O8 B4 -165.4(3) 3_456 . . . ?
K2 B5 O10 Al2 154.3(3) 3_456 . . 3_456 ?
K2 B5 O11 K1 -91.4(8) 3_456 . . 3_556 ?
K2 B5 O11 B6 97.3(7) 3_456 . . . ?
K2 B10 O17 K3 87.20(17) . . . . ?
K2 B10 O17 B9 -138.1(3) . . . . ?
K2 B10 O19 Al1 93.9(7) . . . 3_556 ?
K2 B10 O20 K3 -110.6(5) . . . 1_655 ?
K2 B10 O20 B11 96.7(6) . . . . ?
K3 Al1 O6 K2 111.02(9) 3_456 . . 3_556 ?
K3 Al1 O6 B3 -141.8(3) 3_456 . . . ?
K3 Al1 O6 B4 10.4(4) 3_456 . . . ?
K3 B1 O1 K2 83.57(10) 1_656 . . 1_656 ?
K3 B1 O1 Al1 -138.0(4) 1_656 . . 3_557 ?
K3 B1 O2 K2 -70.48(12) 1_656 . . 1_656 ?
K3 B1 O2 B2 127.0(3) 1_656 . . . ?
K3 B1 O4 K1 27.7(5) 1_656 . . 1_455 ?
K3 B1 O4 B3 -119.6(4) 1_656 . . . ?
K3 B7 O13 K1 -144.64(19) 4_656 . . 1_455 ?
K3 B7 O13 Al2 93.2(2) 4_656 . . . ?
K3 B7 O14 K3 99.6(4) 4_656 . . 4_556 ?
K3 B7 O14 B8 -62.5(4) 4_656 . . . ?
K3 B7 O15 B9 122.8(4) 4_656 . . . ?
K3 B9 O15 K3 177.20(19) . . . 4_656 ?
K3 B9 O15 B7 -124.7(4) 4_656 . . . ?
K3 B9 O15 B7 52.5(5) . . . . ?
K3 B9 O16 K1 96.13(13) . . . 4_455 ?
K3 B9 O16 K1 -83.0(2) 4_656 . . 4_455 ?
K3 B9 O16 K3 -179.13(16) 4_656 . . . ?
K3 B9 O16 B8 -118.0(4) . . . . ?
K3 B9 O16 B8 62.9(4) 4_656 . . . ?
K3 B9 O17 K2 97.4(2) . . . . ?
K3 B9 O17 K2 -83.4(3) 4_656 . . . ?
K3 B9 O17 K3 179.2(2) 4_656 . . . ?
K3 B9 O17 B10 -141.0(4) . . . . ?
K3 B9 O17 B10 38.2(5) 4_656 . . . ?
K3 B9 O18 K1 -42.3(2) . . . 4_455 ?
K3 B9 O18 K1 134.94(13) 4_656 . . 4_455 ?
K3 B9 O18 K3 -177.25(17) . . . 4_656 ?
K3 B9 O18 B11 86.8(4) . . . . ?
K3 B9 O18 B11 -95.9(3) 4_656 . . . ?
K3 B11 O18 K1 -142.33(19) 4_656 . . 4_455 ?
K3 B11 O18 B9 102.0(3) 4_656 . . . ?
K3 B11 O20 K3 125.4(2) 4_656 . . 1_655 ?
K3 B11 O20 B10 -83.5(4) 4_656 . . . ?
K3 B11 O21 B8 -94.3(3) 4_656 . . 1_655 ?
B3 B4 O6 K2 98.0(2) . . . 3_556 ?
B3 B4 O6 Al1 -160.1(4) . . . . ?
B3 B4 O7 K1 94.5(2) . . . 1_455 ?
B3 B4 O7 Al2 -149.7(3) . . . . ?
B3 B4 O8 K2 48.3(6) . . . 3_456 ?
B3 B4 O8 B5 -159.5(3) . . . . ?
B3 B4 O9 K2 -35.1(3) . . . 3_556 ?
B3 B4 O9 B6 158.2(3) . . . . ?
B4 B3 O4 K1 47.3(3) . . . 1_455 ?
B4 B3 O4 B1 -158.4(3) . . . . ?
B4 B3 O5 K1 -69.8(5) . . . . ?
B4 B3 O5 K2 27.5(3) . . . 3_556 ?
B4 B3 O5 B2 159.0(3) . . . . ?
B4 B3 O6 K2 -93.0(2) . . . 3_556 ?
B4 B3 O6 Al1 160.4(4) . . . . ?
B4 B3 O7 K1 -110.3(2) . . . 1_455 ?
B4 B3 O7 Al2 145.0(4) . . . . ?
O1 Al1 O6 K2 157.71(11) 3_557 . . 3_556 ?
O1 Al1 O6 B3 -95.1(3) 3_557 . . . ?
O1 Al1 O6 B4 57.1(4) 3_557 . . . ?
O1 B1 O2 K2 -25.4(4) . . . 1_656 ?
O1 B1 O2 B2 172.1(3) . . . . ?
O1 B1 O4 K1 -39.6(5) . . . 1_455 ?
O1 B1 O4 B3 173.1(4) . . . . ?
O2 B1 O1 K2 21.0(3) . . . 1_656 ?
O2 B1 O1 K3 -62.5(4) . . . 1_656 ?
O2 B1 O1 Al1 159.5(3) . . . 3_557 ?
O2 B1 O4 K1 141.8(3) . . . 1_455 ?
O2 B1 O4 B3 -5.6(5) . . . . ?
O2 B2 O3 K1 145.9(3) . . . . ?
O2 B2 O3 Al1 -2.9(6) . . . 3_657 ?
O2 B2 O5 K1 -150.6(3) . . . . ?
O2 B2 O5 K2 124.6(3) . . . 3_556 ?
O2 B2 O5 B3 4.6(5) . . . . ?
O3 Al1 O6 K2 -79.66(13) 3_657 . . 3_556 ?
O3 Al1 O6 B3 27.5(3) 3_657 . . . ?
O3 Al1 O6 B4 179.8(3) 3_657 . . . ?
O3 B2 O2 K2 31.6(5) . . . 1_656 ?
O3 B2 O2 B1 -171.6(3) . . . . ?
O3 B2 O5 K1 30.7(3) . . . . ?
O3 B2 O5 K2 -54.1(4) . . . 3_556 ?
O3 B2 O5 B3 -174.1(3) . . . . ?
O4 B1 O1 K2 -157.6(4) . . . 1_656 ?
O4 B1 O1 K3 118.8(4) . . . 1_656 ?
O4 B1 O1 Al1 -19.1(6) . . . 3_557 ?
O4 B1 O2 K2 153.3(3) . . . 1_656 ?
O4 B1 O2 B2 -9.2(5) . . . . ?
O4 B3 O5 K1 113.1(4) . . . . ?
O4 B3 O5 K2 -149.6(3) . . . 3_556 ?
O4 B3 O5 B2 -18.1(5) . . . . ?
O4 B3 O6 K2 152.6(2) . . . 3_556 ?
O4 B3 O6 Al1 46.0(4) . . . . ?
O4 B3 O6 B4 -114.4(3) . . . . ?
O4 B3 O7 K1 3.7(3) . . . 1_455 ?
O4 B3 O7 Al2 -101.0(4) . . . . ?
O4 B3 O7 B4 114.0(3) . . . . ?
O5 B2 O2 K2 -147.1(3) . . . 1_656 ?
O5 B2 O2 B1 9.7(5) . . . . ?
O5 B2 O3 K1 -35.4(4) . . . . ?
O5 B2 O3 Al1 175.8(2) . . . 3_657 ?
O5 B3 O4 K1 -135.5(3) . . . 1_455 ?
O5 B3 O4 B1 18.8(5) . . . . ?
O5 B3 O6 K2 22.0(3) . . . 3_556 ?
O5 B3 O6 Al1 -84.6(4) . . . . ?
O5 B3 O6 B4 115.0(3) . . . . ?
O5 B3 O7 K1 136.4(3) . . . 1_455 ?
O5 B3 O7 Al2 31.7(5) . . . . ?
O5 B3 O7 B4 -113.3(3) . . . . ?
O6 B3 O4 K1 96.1(3) . . . 1_455 ?
O6 B3 O4 B1 -109.6(4) . . . . ?
O6 B3 O5 K1 -118.5(3) . . . . ?
O6 B3 O5 K2 -21.2(3) . . . 3_556 ?
O6 B3 O5 B2 110.3(4) . . . . ?
O6 B3 O7 K1 -109.9(2) . . . 1_455 ?
O6 B3 O7 Al2 145.5(3) . . . . ?
O6 B3 O7 B4 0.4(3) . . . . ?
O6 B4 O7 K1 94.0(2) . . . 1_455 ?
O6 B4 O7 Al2 -150.2(2) . . . . ?
O6 B4 O7 B3 -0.4(3) . . . . ?
O6 B4 O8 K2 -3.3(6) . . . 3_456 ?
O6 B4 O8 B5 148.9(3) . . . . ?
O6 B4 O9 K2 16.2(3) . . . 3_556 ?
O6 B4 O9 B6 -150.6(3) . . . . ?
O7 Al2 O13 K1 25.13(12) . . . 1_455 ?
O7 Al2 O13 B7 165.7(3) . . . . ?
O7 B3 O4 K1 -4.0(3) . . . 1_455 ?
O7 B3 O4 B1 150.3(3) . . . . ?
O7 B3 O5 K1 -17.8(6) . . . . ?
O7 B3 O5 K2 79.5(3) . . . 3_556 ?
O7 B3 O5 B2 -149.0(3) . . . . ?
O7 B3 O6 K2 -93.4(2) . . . 3_556 ?
O7 B3 O6 Al1 160.0(2) . . . . ?
O7 B3 O6 B4 -0.4(3) . . . . ?
O7 B4 O6 K2 98.4(2) . . . 3_556 ?
O7 B4 O6 Al1 -159.6(3) . . . . ?
O7 B4 O6 B3 0.4(3) . . . . ?
O7 B4 O8 K2 97.7(4) . . . 3_456 ?
O7 B4 O8 B5 -110.2(4) . . . . ?
O7 B4 O9 K2 -84.0(3) . . . 3_556 ?
O7 B4 O9 B6 109.2(4) . . . . ?
O8 B4 O6 K2 -147.0(3) . . . 3_556 ?
O8 B4 O6 Al1 -45.0(5) . . . . ?
O8 B4 O6 B3 115.1(3) . . . . ?
O8 B4 O7 K1 -21.6(3) . . . 1_455 ?
O8 B4 O7 Al2 94.2(4) . . . . ?
O8 B4 O7 B3 -116.0(3) . . . . ?
O8 B4 O9 K2 147.5(3) . . . 3_556 ?
O8 B4 O9 B6 -19.3(5) . . . . ?
O8 B5 O10 K2 24.3(4) . . . 3_456 ?
O8 B5 O10 Al2 178.6(3) . . . 3_456 ?
O8 B5 O11 K1 169.0(2) . . . 3_556 ?
O8 B5 O11 B6 -2.4(6) . . . . ?
O9 B4 O6 K2 -15.1(3) . . . 3_556 ?
O9 B4 O6 Al1 86.9(4) . . . . ?
O9 B4 O6 B3 -113.0(3) . . . . ?
O9 B4 O7 K1 -151.3(2) . . . 1_455 ?
O9 B4 O7 Al2 -35.5(4) . . . . ?
O9 B4 O7 B3 114.2(3) . . . . ?
O9 B4 O8 K2 -134.2(3) . . . 3_456 ?
O9 B4 O8 B5 17.9(5) . . . . ?
O9 B6 O11 K1 -172.7(3) . . . 3_556 ?
O9 B6 O11 B5 1.3(5) . . . . ?
O9 B6 O12 K1 173.3(4) . . . 3_556 ?
O9 B6 O12 Al2 3.4(6) . . . 3_556 ?
O10 Al2 O7 K1 87.09(12) 3_456 . . 1_455 ?
O10 Al2 O7 B3 -169.2(3) 3_456 . . . ?
O10 Al2 O7 B4 -34.6(3) 3_456 . . . ?
O10 Al2 O13 K1 -87.19(12) 3_456 . . 1_455 ?
O10 Al2 O13 B7 53.4(3) 3_456 . . . ?
O10 B5 O8 K2 -22.8(4) . . . 3_456 ?
O10 B5 O8 B4 171.8(3) . . . . ?
O10 B5 O11 K1 -10.8(6) . . . 3_556 ?
O10 B5 O11 B6 177.9(3) . . . . ?
O11 B5 O8 K2 157.5(4) . . . 3_456 ?
O11 B5 O8 B4 -7.9(6) . . . . ?
O11 B5 O10 K2 -156.0(3) . . . 3_456 ?
O11 B5 O10 Al2 -1.7(6) . . . 3_456 ?
O11 B6 O9 K2 -151.4(3) . . . 3_556 ?
O11 B6 O9 B4 10.2(5) . . . . ?
O11 B6 O12 K1 -6.4(4) . . . 3_556 ?
O11 B6 O12 Al2 -176.3(3) . . . 3_556 ?
O12 Al2 O7 K1 -152.49(11) 3_556 . . 1_455 ?
O12 Al2 O7 B3 -48.8(4) 3_556 . . . ?
O12 Al2 O7 B4 85.8(3) 3_556 . . . ?
O12 Al2 O13 K1 148.10(11) 3_556 . . 1_455 ?
O12 Al2 O13 B7 -71.3(3) 3_556 . . . ?
O12 B6 O9 K2 28.9(6) . . . 3_556 ?
O12 B6 O9 B4 -169.5(4) . . . . ?
O12 B6 O11 K1 7.0(4) . . . 3_556 ?
O12 B6 O11 B5 -179.0(4) . . . . ?
O13 Al2 O7 K1 -26.64(13) . . . 1_455 ?
O13 Al2 O7 B3 77.0(3) . . . . ?
O13 Al2 O7 B4 -148.4(3) . . . . ?
O13 B7 O14 K3 -22.9(6) . . . 4_556 ?
O13 B7 O14 B8 175.0(4) . . . . ?
O13 B7 O15 K3 69.7(4) . . . 4_656 ?
O13 B7 O15 B9 -167.5(3) . . . . ?
O14 B7 O13 K1 -9.3(6) . . . 1_455 ?
O14 B7 O13 Al2 -131.4(3) . . . . ?
O14 B7 O15 K3 -112.3(3) . . . 4_656 ?
O14 B7 O15 B9 10.6(6) . . . . ?
O14 B8 O16 K1 140.7(3) . . . 4_455 ?
O14 B8 O16 K3 -111.9(4) . . . . ?
O14 B8 O16 B9 1.4(6) . . . . ?
O15 B7 O13 K1 168.7(2) . . . 1_455 ?
O15 B7 O13 Al2 46.6(5) . . . . ?
O15 B7 O14 K3 159.1(3) . . . 4_556 ?
O15 B7 O14 B8 -3.1(6) . . . . ?
O15 B9 O16 K1 -141.0(2) . . . 4_455 ?
O15 B9 O16 K3 122.9(3) . . . . ?
O15 B9 O16 B8 4.9(5) . . . . ?
O15 B9 O17 K2 -26.7(4) . . . . ?
O15 B9 O17 K3 -124.1(3) . . . . ?
O15 B9 O17 B10 95.0(4) . . . . ?
O15 B9 O18 K1 140.7(3) . . . 4_455 ?
O15 B9 O18 K3 5.7(3) . . . 4_656 ?
O15 B9 O18 B11 -90.2(4) . . . . ?
O16 B8 O14 K3 -170.7(3) . . . 4_556 ?
O16 B8 O14 B7 -2.7(6) . . . . ?
O16 B9 O15 K3 113.6(3) . . . 4_656 ?
O16 B9 O15 B7 -11.1(5) . . . . ?
O16 B9 O17 K2 94.6(3) . . . . ?
O16 B9 O17 K3 -2.8(3) . . . . ?
O16 B9 O17 B10 -143.7(3) . . . . ?
O16 B9 O18 K1 20.0(3) . . . 4_455 ?
O16 B9 O18 K3 -114.9(3) . . . 4_656 ?
O16 B9 O18 B11 149.2(3) . . . . ?
O17 B9 O15 K3 -126.6(2) . . . 4_656 ?
O17 B9 O15 B7 108.7(4) . . . . ?
O17 B9 O16 K1 98.7(3) . . . 4_455 ?
O17 B9 O16 K3 2.6(3) . . . . ?
O17 B9 O16 B8 -115.4(4) . . . . ?
O17 B9 O18 K1 -99.7(3) . . . 4_455 ?
O17 B9 O18 K3 125.4(3) . . . 4_656 ?
O17 B9 O18 B11 29.5(5) . . . . ?
O17 B10 O19 K2 34.6(4) . . . . ?
O17 B10 O19 Al1 128.5(6) . . . 3_556 ?
O17 B10 O20 K3 159.5(3) . . . 1_655 ?
O17 B10 O20 B11 6.8(6) . . . . ?
O18 B9 O15 K3 -6.0(3) . . . 4_656 ?
O18 B9 O15 B7 -130.7(4) . . . . ?
O18 B9 O16 K1 -22.4(3) . . . 4_455 ?
O18 B9 O16 K3 -118.5(3) . . . . ?
O18 B9 O16 B8 123.5(4) . . . . ?
O18 B9 O17 K2 -145.2(2) . . . . ?
O18 B9 O17 K3 117.4(3) . . . . ?
O18 B9 O17 B10 -23.6(5) . . . . ?
O18 B11 O20 K3 -151.3(3) . . . 1_655 ?
O18 B11 O20 B10 -0.2(6) . . . . ?
O18 B11 O21 K3 -49.4(4) . . . 4_656 ?
O18 B11 O21 B8 -143.7(4) . . . 1_655 ?
O19 Al1 O6 K2 37.06(12) 3_556 . . 3_556 ?
O19 Al1 O6 B3 144.3(3) 3_556 . . . ?
O19 Al1 O6 B4 -63.5(4) 3_556 . . . ?
O19 B10 O17 K2 -35.1(4) . . . . ?
O19 B10 O17 K3 52.1(5) . . . . ?
O19 B10 O17 B9 -173.1(4) . . . . ?
O19 B10 O20 K3 -20.7(4) . . . 1_655 ?
O19 B10 O20 B11 -173.5(4) . . . . ?
O20 B10 O17 K2 144.6(3) . . . . ?
O20 B10 O17 K3 -128.2(3) . . . . ?
O20 B10 O17 B9 6.6(6) . . . . ?
O20 B10 O19 K2 -145.1(3) . . . . ?
O20 B10 O19 Al1 -51.2(9) . . . 3_556 ?
O20 B11 O18 K1 96.4(4) . . . 4_455 ?
O20 B11 O18 K3 -121.3(4) . . . 4_656 ?
O20 B11 O18 B9 -19.2(6) . . . . ?
O20 B11 O21 K3 125.4(4) . . . 4_656 ?
O20 B11 O21 B8 31.1(6) . . . 1_655 ?
O21 B8 O14 K3 10.8(4) 1_455 . . 4_556 ?
O21 B8 O14 B7 178.7(3) 1_455 . . . ?
O21 B8 O16 K1 -40.8(5) 1_455 . . 4_455 ?
O21 B8 O16 K3 66.6(4) 1_455 . . . ?
O21 B8 O16 B9 179.9(3) 1_455 . . . ?
O21 B11 O18 K1 -89.1(4) . . . 4_455 ?
O21 B11 O18 K3 53.3(4) . . . 4_656 ?
O21 B11 O18 B9 155.3(4) . . . . ?
O21 B11 O20 K3 34.1(5) . . . 1_655 ?
O21 B11 O20 B10 -174.9(3) . . . . ?

_olex2_submission_special_instructions 'No special instructions were received'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_111
_database_code_depnum_ccdc_archive 'CCDC 2371100'
loop_
_audit_author_name
_audit_author_address
'Haoran Wang'
;Xinjiang Technical Institute of Physics and Chemistry
China
;
_audit_update_record             
;
2024-07-16 deposited with the CCDC.	2024-08-12 downloaded from the CCDC.
;
_audit_creation_date             2022-12-01
_audit_creation_method           
;
Olex2 1.3
(compiled 2020.11.12 svn.r5f609507 for OlexSys, GUI svn.r6408)
;
_shelx_SHELXL_version_number     2016/6
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'Al2 B9 K3 Mo O21'
_chemical_formula_sum            'Al2 B9 K3 Mo O21'
_chemical_formula_weight         700.49
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Al Al 0.0645 0.0514 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
B B 0.0013 0.0007 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_H-M_alt        'P -1'
_space_group_name_Hall           '-P 1'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   7.0548(11)
_cell_length_b                   11.9155(18)
_cell_length_c                   12.2046(18)
_cell_angle_alpha                77.269(6)
_cell_angle_beta                 78.861(7)
_cell_angle_gamma                89.456(6)
_cell_volume                     981.3(3)
_cell_formula_units_Z            2
_cell_measurement_reflns_used    9545
_cell_measurement_temperature    293.15
_cell_measurement_theta_max      27.55
_cell_measurement_theta_min      2.74
_shelx_estimated_absorpt_T_max   0.862
_shelx_estimated_absorpt_T_min   0.687
_exptl_absorpt_coefficient_mu    1.498
_exptl_absorpt_correction_T_max  0.7456
_exptl_absorpt_correction_T_min  0.5657
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
;
SADABS-2016/2 (Bruker,2016/2) was used for absorption correction.
wR2(int) was 0.1294 before and 0.0732 after correction.
The Ratio of minimum to maximum transmission is 0.7587.
The λ/2 correction factor is Not present.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            'clear light colourless'
_exptl_crystal_colour_lustre     clear
_exptl_crystal_colour_modifier   light
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    2.371
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       block
_exptl_crystal_F_000             676
_exptl_crystal_size_max          0.271
_exptl_crystal_size_mid          0.149
_exptl_crystal_size_min          0.102
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0564
_diffrn_reflns_av_unetI/netI     0.0337
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.997
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            37235
_diffrn_reflns_point_group_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.584
_diffrn_reflns_theta_min         1.753
_diffrn_ambient_temperature      293.15
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  'Bruker D8 Venture'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_diffrn_source_current           1.4
_diffrn_source_power             0.07
_diffrn_source_voltage           50.0
_diffrn_standards_number         0
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                3880
_reflns_number_total             4530
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'SAINT V8.38A (Bruker, 2018)'
_computing_data_collection       ?
_computing_data_reduction        'SAINT V8.38A (Bruker, 2018)'
_computing_molecular_graphics    'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_structure_refinement  'XL  (Sheldrick, 2008)'
_computing_structure_solution    'SHELXT 2014/5 (Sheldrick, 2014)'
_refine_diff_density_max         1.314
_refine_diff_density_min         -0.718
_refine_diff_density_rms         0.111
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.069
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     325
_refine_ls_number_reflns         4530
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0406
_refine_ls_R_factor_gt           0.0336
_refine_ls_restrained_S_all      1.069
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0354P)²+1.4364P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0819
_refine_ls_wR_factor_ref         0.0848
_refine_special_details          ?
_olex2_refinement_description    
;
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
K1 K 0.16744(9) 1.01459(6) 0.83948(7) 0.03141(16) Uani 1 1 d . . . . .
K2 K 0.66108(9) 0.50524(5) 0.84739(6) 0.02496(14) Uani 1 1 d . . . . .
K3 K -0.25056(12) 0.08492(6) 0.56664(7) 0.04095(19) Uani 1 1 d . . . . .
Al1 Al 0.16508(10) 0.66330(6) 0.80431(7) 0.01426(16) Uani 1 1 d . . . . .
Al2 Al 0.33095(10) 0.81141(6) 0.15208(7) 0.01558(16) Uani 1 1 d . . . . .
Mo1 Mo 0.31410(4) 0.19608(2) 0.48677(3) 0.03338(9) Uani 1 1 d . . . . .
B1 B 0.6104(4) 0.9547(2) 0.8420(3) 0.0179(6) Uani 1 1 d . . . . .
B2 B 0.5189(4) 0.7633(2) 0.8298(3) 0.0185(6) Uani 1 1 d . . . . .
B3 B 0.8590(4) 0.8188(2) 0.8051(3) 0.0192(6) Uani 1 1 d . . . . .
B4 B 0.2130(5) 0.5861(3) 0.5853(3) 0.0254(7) Uani 1 1 d . . . . .
B5 B 0.2766(5) 0.4619(3) 0.4526(3) 0.0283(7) Uani 1 1 d . . . . .
B6 B 0.2488(5) 0.6644(3) 0.3805(3) 0.0274(7) Uani 1 1 d . . . . .
B7 B 0.0040(4) 0.7523(2) 0.0812(3) 0.0174(6) Uani 1 1 d . . . . .
B8 B -0.3223(4) 0.6964(2) 0.0783(3) 0.0157(5) Uani 1 1 d . . . . .
B9 B -0.0596(4) 0.5670(2) 0.0405(3) 0.0152(5) Uani 1 1 d . . . . .
O1 O 0.5551(3) 1.05696(15) 0.85875(18) 0.0231(4) Uani 1 1 d . . . . .
O2 O 0.4715(2) 0.87104(15) 0.84861(18) 0.0216(4) Uani 1 1 d . . . . .
O3 O 0.3917(2) 0.68120(15) 0.83281(17) 0.0209(4) Uani 1 1 d . . . . .
O4 O 0.8042(2) 0.93020(15) 0.81153(18) 0.0232(4) Uani 1 1 d . . . . .
O5 O 0.7152(2) 0.73865(15) 0.81009(18) 0.0230(4) Uani 1 1 d . . . . .
O6 O 1.0429(2) 0.79157(15) 0.79895(18) 0.0221(4) Uani 1 1 d . . . . .
O7 O 0.1787(3) 0.60008(19) 0.69069(18) 0.0322(5) Uani 1 1 d . . . . .
O8 O 0.2460(4) 0.47729(18) 0.56169(19) 0.0353(5) Uani 1 1 d . . . . .
O9 O 0.2190(4) 0.67693(18) 0.49265(19) 0.0364(5) Uani 1 1 d . . . . .
O10 O 0.2498(3) 0.75579(19) 0.29695(19) 0.0331(5) Uani 1 1 d . . . . .
O11 O 0.2765(3) 0.55400(17) 0.36187(18) 0.0303(5) Uani 1 1 d . . . . .
O12 O 0.3077(4) 0.35742(19) 0.4283(2) 0.0419(6) Uani 1 1 d . . . . .
O13 O 0.3366(5) 0.1625(3) 0.6261(3) 0.0689(9) Uani 1 1 d . . . . .
O14 O 0.1143(4) 0.1251(2) 0.4702(3) 0.0671(10) Uani 1 1 d . . . . .
O15 O 0.5078(4) 0.1400(2) 0.4109(2) 0.0472(6) Uani 1 1 d . . . . .
O16 O 0.1258(2) 0.83402(15) 0.09021(18) 0.0211(4) Uani 1 1 d . . . . .
O17 O -0.1865(2) 0.78039(15) 0.07741(18) 0.0220(4) Uani 1 1 d . . . . .
O18 O 0.0594(2) 0.64274(15) 0.07603(16) 0.0175(4) Uani 1 1 d . . . . .
O19 O -0.0225(2) 0.44197(14) 0.08328(15) 0.0146(3) Uani 1 1 d . . . . .
O20 O -0.2610(2) 0.59155(15) 0.05843(16) 0.0168(4) Uani 1 1 d . . . . .
O21 O -0.5104(2) 0.71724(15) 0.09538(18) 0.0208(4) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
K1 K1 4.1101(16) 2_577 ?
K1 B1 3.203(3) . ?
K1 B3 3.352(3) 1_455 ?
K1 B7 3.284(3) 2_576 ?
K1 O1 2.8489(19) . ?
K1 O2 2.7344(19) . ?
K1 O4 2.8693(19) 1_455 ?
K1 O6 2.9782(19) 1_455 ?
K1 O13 2.852(3) 1_565 ?
K1 O16 2.8628(19) 2_576 ?
K1 O16 3.293(2) 1_556 ?
K1 O17 2.8576(19) 2_576 ?
K2 B2 3.200(3) . ?
K2 B8 3.259(3) 2_566 ?
K2 B9 3.382(3) 2_666 ?
K2 O3 2.8161(18) . ?
K2 O5 2.7355(19) . ?
K2 O11 2.751(2) 2_666 ?
K2 O12 3.368(3) 2_666 ?
K2 O18 2.7911(18) 2_666 ?
K2 O19 2.9513(18) 2_666 ?
K2 O20 2.9735(18) 2_566 ?
K2 O20 3.1175(19) 1_656 ?
K2 O21 2.7560(19) 2_566 ?
K3 Mo1 3.5564(10) 1_455 ?
K3 Mo1 3.5972(9) 2_556 ?
K3 B1 3.335(3) 1_445 ?
K3 B6 3.192(3) 2_566 ?
K3 O4 3.238(2) 1_445 ?
K3 O9 2.770(2) 2_566 ?
K3 O10 2.787(2) 2_566 ?
K3 O13 3.048(4) 1_455 ?
K3 O14 2.616(3) . ?
K3 O14 2.769(3) 2_556 ?
K3 O15 3.183(3) 2_556 ?
K3 O15 2.763(3) 1_455 ?
Al1 O3 1.7250(19) . ?
Al1 O6 1.7424(19) 1_455 ?
Al1 O7 1.705(2) . ?
Al1 O19 1.7889(19) 2_566 ?
Al2 O1 1.7365(19) 2_676 ?
Al2 O10 1.730(2) . ?
Al2 O16 1.7501(19) . ?
Al2 O21 1.7347(19) 1_655 ?
Mo1 O12 1.901(2) . ?
Mo1 O13 1.697(3) . ?
Mo1 O14 1.718(3) . ?
Mo1 O15 1.714(3) . ?
B1 O1 1.322(3) . ?
B1 O2 1.383(3) . ?
B1 O4 1.392(3) . ?
B2 O2 1.380(3) . ?
B2 O3 1.324(3) . ?
B2 O5 1.398(3) . ?
B3 O4 1.393(3) . ?
B3 O5 1.384(3) . ?
B3 O6 1.326(3) . ?
B4 O7 1.309(4) . ?
B4 O8 1.396(4) . ?
B4 O9 1.377(4) . ?
B5 O8 1.360(4) . ?
B5 O11 1.376(4) . ?
B5 O12 1.348(4) . ?
B6 O9 1.385(4) . ?
B6 O10 1.317(4) . ?
B6 O11 1.389(4) . ?
B7 O16 1.341(3) . ?
B7 O17 1.389(3) . ?
B7 O18 1.370(3) . ?
B8 O17 1.389(3) . ?
B8 O20 1.375(3) . ?
B8 O21 1.333(3) . ?
B9 O18 1.426(3) . ?
B9 O19 1.537(3) 2_565 ?
B9 O19 1.505(3) . ?
B9 O20 1.433(3) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
B1 K1 K1 113.63(6) . 2_577 ?
B1 K1 B3 120.31(7) . 1_455 ?
B1 K1 B7 119.61(7) . 2_576 ?
B1 K1 O16 79.08(7) . 1_556 ?
B3 K1 K1 86.14(6) 1_455 2_577 ?
B7 K1 K1 60.77(6) 2_576 2_577 ?
B7 K1 B3 119.07(7) 2_576 1_455 ?
B7 K1 O16 100.65(7) 2_576 1_556 ?
O1 K1 K1 106.65(5) . 2_577 ?
O1 K1 B1 24.35(6) . . ?
O1 K1 B3 144.63(6) . 1_455 ?
O1 K1 B7 95.54(6) . 2_576 ?
O1 K1 O4 168.90(6) . 1_455 ?
O1 K1 O6 121.46(5) . 1_455 ?
O1 K1 O13 75.22(9) . 1_565 ?
O1 K1 O16 86.30(6) . 1_556 ?
O1 K1 O16 119.04(6) . 2_576 ?
O1 K1 O17 70.74(5) . 2_576 ?
O2 K1 K1 110.40(5) . 2_577 ?
O2 K1 B1 25.40(6) . . ?
O2 K1 B3 95.36(6) . 1_455 ?
O2 K1 B7 142.07(7) . 2_576 ?
O2 K1 O1 49.36(5) . . ?
O2 K1 O4 119.69(6) . 1_455 ?
O2 K1 O6 72.39(5) . 1_455 ?
O2 K1 O13 95.58(9) . 1_565 ?
O2 K1 O16 159.34(7) . 2_576 ?
O2 K1 O16 67.76(6) . 1_556 ?
O2 K1 O17 117.68(6) . 2_576 ?
O4 K1 K1 77.90(5) 1_455 2_577 ?
O4 K1 B1 144.56(7) 1_455 . ?
O4 K1 B3 24.34(6) 1_455 1_455 ?
O4 K1 B7 95.50(6) 1_455 2_576 ?
O4 K1 O6 47.46(5) 1_455 1_455 ?
O4 K1 O16 90.51(6) 1_455 1_556 ?
O6 K1 K1 97.38(5) 1_455 2_577 ?
O6 K1 B1 97.12(6) 1_455 . ?
O6 K1 B3 23.24(6) 1_455 1_455 ?
O6 K1 B7 142.02(6) 1_455 2_576 ?
O6 K1 O16 75.60(5) 1_455 1_556 ?
O13 K1 K1 147.34(7) 1_565 2_577 ?
O13 K1 B1 81.86(10) 1_565 . ?
O13 K1 B3 111.51(10) 1_565 1_455 ?
O13 K1 B7 86.58(9) 1_565 2_576 ?
O13 K1 O4 106.63(9) 1_565 1_455 ?
O13 K1 O6 109.45(8) 1_565 1_455 ?
O13 K1 O16 160.78(9) 1_565 1_556 ?
O13 K1 O16 97.05(8) 1_565 2_576 ?
O13 K1 O17 82.86(8) 1_565 2_576 ?
O16 K1 K1 43.79(3) 1_556 2_577 ?
O16 K1 K1 52.74(4) 2_576 2_577 ?
O16 K1 B1 142.50(7) 2_576 . ?
O16 K1 B3 80.68(7) 1_556 1_455 ?
O16 K1 B3 95.14(6) 2_576 1_455 ?
O16 K1 B7 23.96(6) 2_576 2_576 ?
O16 K1 O4 71.87(5) 2_576 1_455 ?
O16 K1 O6 118.06(5) 2_576 1_455 ?
O16 K1 O16 96.53(5) 2_576 1_556 ?
O17 K1 K1 67.88(5) 2_576 2_577 ?
O17 K1 B1 94.70(6) 2_576 . ?
O17 K1 B3 143.06(7) 2_576 1_455 ?
O17 K1 B7 24.92(6) 2_576 2_576 ?
O17 K1 O4 120.22(5) 2_576 1_455 ?
O17 K1 O6 163.99(6) 2_576 1_455 ?
O17 K1 O16 48.35(5) 2_576 2_576 ?
O17 K1 O16 96.18(6) 2_576 1_556 ?
B2 K2 B8 116.07(7) . 2_566 ?
B2 K2 B9 118.02(7) . 2_666 ?
B2 K2 O12 69.29(7) . 2_666 ?
B8 K2 B9 114.04(7) 2_566 2_666 ?
B8 K2 O12 110.54(7) 2_566 2_666 ?
O3 K2 B2 24.37(6) . . ?
O3 K2 B8 92.49(6) . 2_566 ?
O3 K2 B9 139.61(6) . 2_666 ?
O3 K2 O12 70.31(6) . 2_666 ?
O3 K2 O19 116.21(5) . 2_666 ?
O3 K2 O20 69.31(5) . 2_566 ?
O3 K2 O20 84.57(5) . 1_656 ?
O5 K2 B2 25.75(6) . . ?
O5 K2 B8 141.80(6) . 2_566 ?
O5 K2 B9 96.81(6) . 2_666 ?
O5 K2 O3 49.73(5) . . ?
O5 K2 O11 108.16(7) . 2_666 ?
O5 K2 O12 66.42(6) . 2_666 ?
O5 K2 O18 120.60(6) . 2_666 ?
O5 K2 O19 70.46(5) . 2_666 ?
O5 K2 O20 117.32(5) . 2_566 ?
O5 K2 O20 65.53(6) . 1_656 ?
O5 K2 O21 165.38(6) . 2_566 ?
O11 K2 B2 111.76(7) 2_666 . ?
O11 K2 B8 84.87(7) 2_666 2_566 ?
O11 K2 B9 106.67(7) 2_666 2_666 ?
O11 K2 O3 105.50(6) 2_666 . ?
O11 K2 O12 43.26(6) 2_666 2_666 ?
O11 K2 O18 92.55(6) 2_666 2_666 ?
O11 K2 O19 112.97(6) 2_666 2_666 ?
O11 K2 O20 99.78(6) 2_666 2_566 ?
O11 K2 O20 160.66(6) 2_666 1_656 ?
O11 K2 O21 77.95(6) 2_666 2_566 ?
O12 K2 B9 121.73(7) 2_666 2_666 ?
O18 K2 B2 142.35(7) 2_666 . ?
O18 K2 B8 93.57(6) 2_666 2_566 ?
O18 K2 B9 24.39(6) 2_666 2_666 ?
O18 K2 O3 161.41(6) 2_666 . ?
O18 K2 O12 123.35(6) 2_666 2_666 ?
O18 K2 O19 50.30(5) 2_666 2_666 ?
O18 K2 O20 112.59(6) 2_666 2_566 ?
O18 K2 O20 76.85(5) 2_666 1_656 ?
O19 K2 B2 92.80(6) 2_666 . ?
O19 K2 B8 138.26(6) 2_666 2_566 ?
O19 K2 B9 26.38(6) 2_666 2_666 ?
O19 K2 O12 107.56(6) 2_666 2_666 ?
O19 K2 O20 142.31(6) 2_666 2_566 ?
O19 K2 O20 47.94(5) 2_666 1_656 ?
O20 K2 B2 91.85(6) 2_566 . ?
O20 K2 B2 71.06(7) 1_656 . ?
O20 K2 B8 24.95(6) 2_566 2_566 ?
O20 K2 B8 111.58(6) 1_656 2_566 ?
O20 K2 B9 127.09(6) 2_566 2_666 ?
O20 K2 B9 58.10(6) 1_656 2_666 ?
O20 K2 O12 109.05(6) 2_566 2_666 ?
O20 K2 O12 131.33(5) 1_656 2_666 ?
O20 K2 O20 99.23(5) 2_566 1_656 ?
O21 K2 B2 139.78(7) 2_566 . ?
O21 K2 B8 23.77(6) 2_566 2_566 ?
O21 K2 B9 93.96(6) 2_566 2_666 ?
O21 K2 O3 116.22(5) 2_566 . ?
O21 K2 O12 115.57(6) 2_566 2_666 ?
O21 K2 O18 71.37(5) 2_566 2_666 ?
O21 K2 O19 120.14(5) 2_566 2_666 ?
O21 K2 O20 112.85(6) 2_566 1_656 ?
O21 K2 O20 48.07(5) 2_566 2_566 ?
Mo1 K3 Mo1 95.97(2) 1_455 2_556 ?
B1 K3 Mo1 103.56(5) 1_445 1_455 ?
B1 K3 Mo1 84.94(5) 1_445 2_556 ?
B6 K3 Mo1 77.97(7) 2_566 1_455 ?
B6 K3 Mo1 173.19(7) 2_566 2_556 ?
B6 K3 B1 93.39(8) 2_566 1_445 ?
B6 K3 O4 100.05(7) 2_566 1_445 ?
O4 K3 Mo1 127.82(4) 1_445 1_455 ?
O4 K3 Mo1 81.12(4) 1_445 2_556 ?
O4 K3 B1 24.39(6) 1_445 1_445 ?
O9 K3 Mo1 70.63(6) 2_566 1_455 ?
O9 K3 Mo1 154.44(6) 2_566 2_556 ?
O9 K3 B1 118.82(7) 2_566 1_445 ?
O9 K3 B6 25.62(8) 2_566 2_566 ?
O9 K3 O4 124.38(6) 2_566 1_445 ?
O9 K3 O10 49.68(7) 2_566 2_566 ?
O9 K3 O13 75.47(8) 2_566 1_455 ?
O9 K3 O14 149.02(9) 2_566 2_556 ?
O9 K3 O15 147.07(8) 2_566 2_556 ?
O10 K3 Mo1 155.12(5) 2_566 2_556 ?
O10 K3 Mo1 90.53(5) 2_566 1_455 ?
O10 K3 B1 70.18(7) 2_566 1_445 ?
O10 K3 B6 24.25(8) 2_566 2_566 ?
O10 K3 O4 75.98(6) 2_566 1_445 ?
O10 K3 O13 72.17(8) 2_566 1_455 ?
O10 K3 O15 133.66(7) 2_566 2_556 ?
O13 K3 Mo1 28.46(6) 1_455 1_455 ?
O13 K3 Mo1 103.39(7) 1_455 2_556 ?
O13 K3 B1 76.91(8) 1_455 1_445 ?
O13 K3 B6 69.80(9) 1_455 2_566 ?
O13 K3 O4 101.22(7) 1_455 1_445 ?
O13 K3 O15 76.39(8) 1_455 2_556 ?
O14 K3 Mo1 99.14(7) . 2_556 ?
O14 K3 Mo1 122.21(7) 2_556 1_455 ?
O14 K3 Mo1 27.59(6) 2_556 2_556 ?
O14 K3 Mo1 132.95(8) . 1_455 ?
O14 K3 B1 87.23(10) 2_556 1_445 ?
O14 K3 B1 121.93(10) . 1_445 ?
O14 K3 B6 159.08(9) 2_556 2_566 ?
O14 K3 B6 87.35(9) . 2_566 ?
O14 K3 O4 98.53(9) . 1_445 ?
O14 K3 O4 72.68(9) 2_556 1_445 ?
O14 K3 O9 77.00(8) . 2_566 ?
O14 K3 O10 144.35(9) 2_556 2_566 ?
O14 K3 O10 93.79(9) . 2_566 ?
O14 K3 O13 151.97(9) . 1_455 ?
O14 K3 O13 130.35(9) 2_556 1_455 ?
O14 K3 O14 74.72(9) . 2_556 ?
O14 K3 O15 54.01(7) 2_556 2_556 ?
O14 K3 O15 112.42(11) . 1_455 ?
O14 K3 O15 127.58(8) . 2_556 ?
O15 K3 Mo1 28.05(5) 1_455 1_455 ?
O15 K3 Mo1 81.06(6) 1_455 2_556 ?
O15 K3 Mo1 76.48(5) 2_556 1_455 ?
O15 K3 Mo1 28.46(5) 2_556 2_556 ?
O15 K3 B1 70.15(7) 2_556 1_445 ?
O15 K3 B1 125.32(8) 1_455 1_445 ?
O15 K3 B6 94.61(8) 1_455 2_566 ?
O15 K3 B6 145.06(8) 2_556 2_566 ?
O15 K3 O4 146.28(7) 1_455 1_445 ?
O15 K3 O4 77.80(6) 2_556 1_445 ?
O15 K3 O9 77.34(8) 1_455 2_566 ?
O15 K3 O10 113.44(7) 1_455 2_566 ?
O15 K3 O13 56.01(8) 1_455 1_455 ?
O15 K3 O14 102.08(9) 1_455 2_556 ?
O15 K3 O15 72.91(9) 1_455 2_556 ?
O3 Al1 K2 154.85(7) . 1_455 ?
O3 Al1 O6 109.78(9) . 1_455 ?
O3 Al1 O19 110.79(9) . 2_566 ?
O6 Al1 K2 87.68(6) 1_455 1_455 ?
O6 Al1 O19 106.39(9) 1_455 2_566 ?
O7 Al1 K2 74.22(8) . 1_455 ?
O7 Al1 O3 110.81(11) . . ?
O7 Al1 O6 117.30(11) . 1_455 ?
O7 Al1 O19 101.30(10) . 2_566 ?
O19 Al1 K2 45.08(6) 2_566 1_455 ?
K2 Al2 K3 121.04(3) 2_666 2_566 ?
O1 Al2 K2 152.13(7) 2_676 2_666 ?
O1 Al2 K3 65.85(8) 2_676 2_566 ?
O1 Al2 O16 109.41(9) 2_676 . ?
O10 Al2 K2 80.76(8) . 2_666 ?
O10 Al2 K3 41.43(8) . 2_566 ?
O10 Al2 O1 105.98(11) . 2_676 ?
O10 Al2 O16 106.76(11) . . ?
O10 Al2 O21 109.44(11) . 1_655 ?
O16 Al2 K2 93.76(6) . 2_666 ?
O16 Al2 K3 110.35(7) . 2_566 ?
O21 Al2 K2 42.56(6) 1_655 2_666 ?
O21 Al2 K3 133.65(7) 1_655 2_566 ?
O21 Al2 O1 111.48(9) 1_655 2_676 ?
O21 Al2 O16 113.39(9) 1_655 . ?
K3 Mo1 K3 135.07(3) 1_655 . ?
K3 Mo1 K3 84.03(2) 1_655 2_556 ?
K3 Mo1 K3 67.52(2) 2_556 . ?
O12 Mo1 K3 117.62(8) . 1_655 ?
O12 Mo1 K3 104.76(8) . . ?
O12 Mo1 K3 145.58(8) . 2_556 ?
O13 Mo1 K3 58.89(12) . 1_655 ?
O13 Mo1 K3 92.43(13) . . ?
O13 Mo1 K3 101.42(11) . 2_556 ?
O13 Mo1 O12 112.59(13) . . ?
O13 Mo1 O14 109.93(18) . . ?
O13 Mo1 O15 106.90(15) . . ?
O14 Mo1 K3 24.79(12) . . ?
O14 Mo1 K3 129.91(10) . 1_655 ?
O14 Mo1 K3 48.30(10) . 2_556 ?
O14 Mo1 O12 111.58(13) . . ?
O15 Mo1 K3 49.28(9) . 1_655 ?
O15 Mo1 K3 128.59(9) . . ?
O15 Mo1 K3 62.21(9) . 2_556 ?
O15 Mo1 O12 110.24(12) . . ?
O15 Mo1 O14 105.25(14) . . ?
K1 B1 K3 92.21(8) . 1_665 ?
O1 B1 K1 62.65(13) . . ?
O1 B1 K3 86.29(17) . 1_665 ?
O1 B1 O2 119.2(2) . . ?
O1 B1 O4 122.2(2) . . ?
O2 B1 K1 58.00(12) . . ?
O2 B1 K3 107.49(17) . 1_665 ?
O2 B1 O4 118.6(2) . . ?
O4 B1 K1 164.3(2) . . ?
O4 B1 K3 73.91(15) . 1_665 ?
O2 B2 K2 165.5(2) . . ?
O2 B2 O5 117.3(2) . . ?
O3 B2 K2 61.34(13) . . ?
O3 B2 O2 124.5(2) . . ?
O3 B2 O5 118.1(2) . . ?
O5 B2 K2 58.21(12) . . ?
O4 B3 K1 58.06(12) . 1_655 ?
O5 B3 K1 169.9(2) . 1_655 ?
O5 B3 O4 117.8(2) . . ?
O6 B3 K1 62.38(13) . 1_655 ?
O6 B3 O4 120.0(2) . . ?
O6 B3 O5 122.2(2) . . ?
O7 B4 O8 121.2(3) . . ?
O7 B4 O9 122.1(3) . . ?
O9 B4 O8 116.7(3) . . ?
O8 B5 K2 166.0(2) . 2_666 ?
O8 B5 O11 120.6(3) . . ?
O11 B5 K2 45.48(14) . 2_666 ?
O12 B5 K2 71.82(18) . 2_666 ?
O12 B5 O8 122.1(3) . . ?
O12 B5 O11 117.3(3) . . ?
O9 B6 K3 59.86(15) . 2_566 ?
O9 B6 O11 117.5(3) . . ?
O10 B6 K3 60.38(16) . 2_566 ?
O10 B6 O9 119.5(3) . . ?
O10 B6 O11 122.9(3) . . ?
O11 B6 K3 171.1(2) . 2_566 ?
O16 B7 K1 60.12(13) . 2_576 ?
O16 B7 O17 118.2(2) . . ?
O16 B7 O18 122.8(2) . . ?
O17 B7 K1 60.10(13) . 2_576 ?
O18 B7 K1 165.9(2) . 2_576 ?
O18 B7 O17 118.9(2) . . ?
O17 B8 K2 164.93(19) . 2_566 ?
O20 B8 K2 65.83(13) . 2_566 ?
O20 B8 O17 119.4(2) . . ?
O21 B8 K2 56.45(13) . 2_566 ?
O21 B8 O17 120.9(2) . . ?
O21 B8 O20 119.7(2) . . ?
K2 B9 K2 144.08(8) 2_666 1_454 ?
O18 B9 K2 151.65(18) . 1_454 ?
O18 B9 K2 53.91(11) . 2_666 ?
O18 B9 O19 110.5(2) . 2_565 ?
O18 B9 O19 113.0(2) . . ?
O18 B9 O20 114.8(2) . . ?
O19 B9 K2 55.19(11) 2_565 1_454 ?
O19 B9 K2 60.63(11) . 2_666 ?
O19 B9 K2 98.50(13) 2_565 2_666 ?
O19 B9 K2 92.70(13) . 1_454 ?
O19 B9 O19 90.49(18) . 2_565 ?
O20 B9 K2 148.65(18) . 2_666 ?
O20 B9 K2 61.15(12) . 1_454 ?
O20 B9 O19 112.6(2) . 2_565 ?
O20 B9 O19 113.0(2) . . ?
Al2 O1 K1 127.88(9) 2_676 . ?
B1 O1 K1 93.01(15) . . ?
B1 O1 Al2 135.96(18) . 2_676 ?
B1 O2 K1 96.59(14) . . ?
B2 O2 K1 138.44(16) . . ?
B2 O2 B1 122.2(2) . . ?
Al1 O3 K2 123.13(9) . . ?
B2 O3 K2 94.29(15) . . ?
B2 O3 Al1 140.80(18) . . ?
K1 O4 K3 103.34(6) 1_655 1_665 ?
B1 O4 K1 136.39(16) . 1_655 ?
B1 O4 K3 81.70(15) . 1_665 ?
B1 O4 B3 120.8(2) . . ?
B3 O4 K1 97.61(14) . 1_655 ?
B3 O4 K3 112.47(17) . 1_665 ?
B2 O5 K2 96.04(15) . . ?
B3 O5 K2 139.42(16) . . ?
B3 O5 B2 122.4(2) . . ?
Al1 O6 K1 129.45(9) 1_655 1_655 ?
B3 O6 K1 94.38(15) . 1_655 ?
B3 O6 Al1 134.25(17) . 1_655 ?
B4 O7 Al1 160.7(2) . . ?
B5 O8 B4 121.4(3) . . ?
B4 O9 K3 141.14(19) . 2_566 ?
B4 O9 B6 123.4(2) . . ?
B6 O9 K3 94.52(18) . 2_566 ?
Al2 O10 K3 114.33(11) . 2_566 ?
B6 O10 K3 95.37(19) . 2_566 ?
B6 O10 Al2 144.1(2) . . ?
B5 O11 K2 113.62(18) . 2_666 ?
B5 O11 B6 120.3(2) . . ?
B6 O11 K2 126.05(19) . 2_666 ?
Mo1 O12 K2 127.04(10) . 2_666 ?
B5 O12 K2 85.8(2) . 2_666 ?
B5 O12 Mo1 146.8(2) . . ?
K1 O13 K3 105.95(10) 1_545 1_655 ?
Mo1 O13 K1 140.68(19) . 1_545 ?
Mo1 O13 K3 92.64(13) . 1_655 ?
K3 O14 K3 105.28(9) . 2_556 ?
Mo1 O14 K3 139.23(19) . . ?
Mo1 O14 K3 104.11(13) . 2_556 ?
K3 O15 K3 107.09(9) 1_655 2_556 ?
Mo1 O15 K3 102.67(12) . 1_655 ?
Mo1 O15 K3 89.33(11) . 2_556 ?
K1 O16 K1 83.47(5) 2_576 1_554 ?
Al2 O16 K1 118.04(9) . 1_554 ?
Al2 O16 K1 121.46(9) . 2_576 ?
B7 O16 K1 102.11(16) . 1_554 ?
B7 O16 K1 95.91(15) . 2_576 ?
B7 O16 Al2 126.22(18) . . ?
B7 O17 K1 94.99(14) . 2_576 ?
B7 O17 B8 120.5(2) . . ?
B8 O17 K1 138.90(16) . 2_576 ?
B7 O18 K2 136.72(15) . 2_666 ?
B7 O18 B9 120.7(2) . . ?
B9 O18 K2 101.70(14) . 2_666 ?
Al1 O19 K2 109.49(8) 2_566 2_666 ?
B9 O19 K2 99.50(12) 2_565 2_666 ?
B9 O19 K2 92.99(12) . 2_666 ?
B9 O19 Al1 128.04(15) 2_565 2_566 ?
B9 O19 Al1 129.34(15) . 2_566 ?
B9 O19 B9 89.51(18) . 2_565 ?
K2 O20 K2 80.77(5) 2_566 1_454 ?
B8 O20 K2 89.22(14) . 2_566 ?
B8 O20 K2 121.66(15) . 1_454 ?
B8 O20 B9 120.7(2) . . ?
B9 O20 K2 145.64(15) . 2_566 ?
B9 O20 K2 95.12(14) . 1_454 ?
Al2 O21 K2 112.24(9) 1_455 2_566 ?
B8 O21 K2 99.78(15) . 2_566 ?
B8 O21 Al2 139.50(17) . 1_455 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
K1 B1 O1 Al2 -159.9(3) . . . 2_676 ?
K1 B1 O2 B2 164.4(3) . . . . ?
K1 B1 O4 K1 129.1(6) . . . 1_655 ?
K1 B1 O4 K3 28.5(6) . . . 1_665 ?
K1 B1 O4 B3 -82.8(7) . . . . ?
K1 B3 O4 K3 107.88(11) 1_655 . . 1_665 ?
K1 B3 O4 B1 -158.4(3) 1_655 . . . ?
K1 B3 O5 K2 -101.0(10) 1_655 . . . ?
K1 B3 O5 B2 58.0(11) 1_655 . . . ?
K1 B3 O6 Al1 164.7(3) 1_655 . . 1_655 ?
K1 B7 O16 K1 -84.56(7) 2_576 . . 1_554 ?
K1 B7 O16 Al2 136.6(2) 2_576 . . . ?
K1 B7 O17 B8 -158.3(3) 2_576 . . . ?
K1 B7 O18 K2 -70.5(8) 2_576 . . 2_666 ?
K1 B7 O18 B9 96.7(7) 2_576 . . . ?
K2 Al1 O3 K2 49.7(2) 1_455 . . . ?
K2 Al1 O3 B2 -150.0(3) 1_455 . . . ?
K2 Al1 O7 B4 133.0(7) 1_455 . . . ?
K2 Al2 O10 K3 166.86(10) 2_666 . . 2_566 ?
K2 Al2 O10 B6 23.6(4) 2_666 . . . ?
K2 Al2 O16 K1 141.35(8) 2_666 . . 2_576 ?
K2 Al2 O16 K1 -118.59(7) 2_666 . . 1_554 ?
K2 Al2 O16 B7 14.6(2) 2_666 . . . ?
K2 B2 O2 K1 -131.9(6) . . . . ?
K2 B2 O2 B1 71.8(8) . . . . ?
K2 B2 O3 Al1 -163.6(3) . . . . ?
K2 B2 O5 B3 -166.5(3) . . . . ?
K2 B5 O8 B4 -1.4(11) 2_666 . . . ?
K2 B5 O11 B6 -179.3(3) 2_666 . . . ?
K2 B5 O12 Mo1 -172.6(4) 2_666 . . . ?
K2 B8 O17 K1 -53.2(8) 2_566 . . 2_576 ?
K2 B8 O17 B7 92.7(7) 2_566 . . . ?
K2 B8 O20 K2 78.64(11) 2_566 . . 1_454 ?
K2 B8 O20 B9 -162.2(2) 2_566 . . . ?
K2 B8 O21 Al2 142.5(3) 2_566 . . 1_455 ?
K2 B9 O18 K2 -139.4(3) 1_454 . . 2_666 ?
K2 B9 O18 B7 -171.1(3) 2_666 . . . ?
K2 B9 O18 B7 49.5(5) 1_454 . . . ?
K2 B9 O19 K2 154.66(6) 1_454 . . 2_666 ?
K2 B9 O19 Al1 118.35(18) 2_666 . . 2_566 ?
K2 B9 O19 Al1 -86.99(17) 1_454 . . 2_566 ?
K2 B9 O19 B9 55.18(11) 1_454 . . 2_565 ?
K2 B9 O19 B9 -99.49(13) 2_666 . . 2_565 ?
K2 B9 O20 K2 -150.8(3) 2_666 . . 1_454 ?
K2 B9 O20 K2 -69.7(4) 2_666 . . 2_566 ?
K2 B9 O20 K2 81.1(2) 1_454 . . 2_566 ?
K2 B9 O20 B8 -131.8(2) 1_454 . . . ?
K2 B9 O20 B8 77.5(4) 2_666 . . . ?
K3 Al2 O10 B6 -143.2(5) 2_566 . . . ?
K3 Al2 O16 K1 116.28(7) 2_566 . . 1_554 ?
K3 Al2 O16 K1 16.21(11) 2_566 . . 2_576 ?
K3 Al2 O16 B7 -110.5(2) 2_566 . . . ?
K3 Mo1 O13 K1 -43.6(3) 2_556 . . 1_545 ?
K3 Mo1 O13 K1 23.9(2) . . . 1_545 ?
K3 Mo1 O13 K1 -119.4(3) 1_655 . . 1_545 ?
K3 Mo1 O13 K3 75.77(9) 2_556 . . 1_655 ?
K3 Mo1 O13 K3 143.32(7) . . . 1_655 ?
K3 Mo1 O14 K3 -135.0(3) . . . 2_556 ?
K3 Mo1 O14 K3 -22.1(2) 1_655 . . 2_556 ?
K3 Mo1 O14 K3 135.0(3) 2_556 . . . ?
K3 Mo1 O14 K3 113.0(2) 1_655 . . . ?
K3 Mo1 O15 K3 -107.37(11) 2_556 . . 1_655 ?
K3 Mo1 O15 K3 -13.17(13) . . . 2_556 ?
K3 Mo1 O15 K3 107.37(11) 1_655 . . 2_556 ?
K3 Mo1 O15 K3 -120.54(8) . . . 1_655 ?
K3 B1 O1 K1 94.42(7) 1_665 . . . ?
K3 B1 O1 Al2 -65.4(3) 1_665 . . 2_676 ?
K3 B1 O2 K1 -81.42(11) 1_665 . . . ?
K3 B1 O2 B2 83.0(3) 1_665 . . . ?
K3 B1 O4 K1 100.6(2) 1_665 . . 1_655 ?
K3 B1 O4 B3 -111.3(2) 1_665 . . . ?
K3 B6 O9 B4 -171.1(3) 2_566 . . . ?
K3 B6 O10 Al2 146.8(4) 2_566 . . . ?
O1 Al2 O10 K3 14.60(13) 2_676 . . 2_566 ?
O1 Al2 O10 B6 -128.6(4) 2_676 . . . ?
O1 Al2 O16 K1 -54.40(14) 2_676 . . 2_576 ?
O1 Al2 O16 K1 45.66(12) 2_676 . . 1_554 ?
O1 Al2 O16 B7 178.9(2) 2_676 . . . ?
O1 B1 O2 K1 14.2(3) . . . . ?
O1 B1 O2 B2 178.7(3) . . . . ?
O1 B1 O4 K1 25.8(4) . . . 1_655 ?
O1 B1 O4 K3 -74.9(3) . . . 1_665 ?
O1 B1 O4 B3 173.9(3) . . . . ?
O2 B1 O1 K1 -13.6(3) . . . . ?
O2 B1 O1 Al2 -173.4(2) . . . 2_676 ?
O2 B1 O4 K1 -157.87(18) . . . 1_655 ?
O2 B1 O4 K3 101.5(2) . . . 1_665 ?
O2 B1 O4 B3 -9.8(4) . . . . ?
O2 B2 O3 K2 -164.4(3) . . . . ?
O2 B2 O3 Al1 32.0(5) . . . . ?
O2 B2 O5 K2 164.1(2) . . . . ?
O2 B2 O5 B3 -2.3(4) . . . . ?
O3 Al1 O7 B4 -73.0(7) . . . . ?
O3 B2 O2 K1 -22.3(5) . . . . ?
O3 B2 O2 B1 -178.6(3) . . . . ?
O3 B2 O5 K2 -13.7(3) . . . . ?
O3 B2 O5 B3 179.8(3) . . . . ?
O4 B1 O1 K1 162.8(3) . . . . ?
O4 B1 O1 Al2 2.9(5) . . . 2_676 ?
O4 B1 O2 K1 -162.3(2) . . . . ?
O4 B1 O2 B2 2.2(4) . . . . ?
O4 B3 O5 K2 -163.94(18) . . . . ?
O4 B3 O5 B2 -4.9(4) . . . . ?
O4 B3 O6 K1 7.6(3) . . . 1_655 ?
O4 B3 O6 Al1 172.3(2) . . . 1_655 ?
O5 B2 O2 K1 160.05(18) . . . . ?
O5 B2 O2 B1 3.7(4) . . . . ?
O5 B2 O3 K2 13.3(3) . . . . ?
O5 B2 O3 Al1 -150.3(2) . . . . ?
O5 B3 O4 K1 169.4(2) . . . 1_655 ?
O5 B3 O4 K3 -82.7(3) . . . 1_665 ?
O5 B3 O4 B1 11.0(4) . . . . ?
O5 B3 O6 K1 -169.7(3) . . . 1_655 ?
O5 B3 O6 Al1 -5.0(5) . . . 1_655 ?
O6 Al1 O3 K2 -178.68(10) 1_455 . . . ?
O6 Al1 O3 B2 -18.3(3) 1_455 . . . ?
O6 Al1 O7 B4 54.1(7) 1_455 . . . ?
O6 B3 O4 K1 -8.0(3) . . . 1_655 ?
O6 B3 O4 K3 99.9(3) . . . 1_665 ?
O6 B3 O4 B1 -166.4(3) . . . . ?
O6 B3 O5 K2 13.4(5) . . . . ?
O6 B3 O5 B2 172.5(3) . . . . ?
O7 Al1 O3 K2 -47.52(15) . . . . ?
O7 Al1 O3 B2 112.8(3) . . . . ?
O7 B4 O8 B5 178.3(3) . . . . ?
O7 B4 O9 K3 16.3(5) . . . 2_566 ?
O7 B4 O9 B6 -177.9(3) . . . . ?
O8 B4 O7 Al1 154.5(5) . . . . ?
O8 B4 O9 K3 -163.5(2) . . . 2_566 ?
O8 B4 O9 B6 2.3(5) . . . . ?
O8 B5 O11 K2 -179.4(2) . . . 2_666 ?
O8 B5 O11 B6 1.3(5) . . . . ?
O8 B5 O12 K2 179.6(3) . . . 2_666 ?
O8 B5 O12 Mo1 6.9(7) . . . . ?
O9 B4 O7 Al1 -25.3(9) . . . . ?
O9 B4 O8 B5 -1.9(5) . . . . ?
O9 B6 O10 K3 9.8(3) . . . 2_566 ?
O9 B6 O10 Al2 156.6(3) . . . . ?
O9 B6 O11 K2 179.8(2) . . . 2_666 ?
O9 B6 O11 B5 -0.9(4) . . . . ?
O10 Al2 O16 K1 159.94(9) . . . 1_554 ?
O10 Al2 O16 K1 59.87(13) . . . 2_576 ?
O10 Al2 O16 B7 -66.8(2) . . . . ?
O10 B6 O9 K3 -9.8(3) . . . 2_566 ?
O10 B6 O9 B4 179.1(3) . . . . ?
O10 B6 O11 K2 -0.1(4) . . . 2_666 ?
O10 B6 O11 B5 179.1(3) . . . . ?
O11 B5 O8 B4 0.2(5) . . . . ?
O11 B5 O12 K2 -0.4(3) . . . 2_666 ?
O11 B5 O12 Mo1 -173.0(3) . . . . ?
O11 B6 O9 K3 170.2(3) . . . 2_566 ?
O11 B6 O9 B4 -0.9(5) . . . . ?
O11 B6 O10 K3 -170.3(3) . . . 2_566 ?
O11 B6 O10 Al2 -23.5(6) . . . . ?
O12 Mo1 O13 K1 131.0(2) . . . 1_545 ?
O12 Mo1 O13 K3 -109.59(11) . . . 1_655 ?
O12 Mo1 O14 K3 -78.3(3) . . . . ?
O12 Mo1 O14 K3 146.69(11) . . . 2_556 ?
O12 Mo1 O15 K3 -143.08(9) . . . 2_556 ?
O12 Mo1 O15 K3 109.55(11) . . . 1_655 ?
O12 B5 O8 B4 -179.7(3) . . . . ?
O12 B5 O11 K2 0.5(4) . . . 2_666 ?
O12 B5 O11 B6 -178.8(3) . . . . ?
O13 Mo1 O14 K3 47.4(3) . . . . ?
O13 Mo1 O14 K3 -87.66(17) . . . 2_556 ?
O13 Mo1 O15 K3 -13.13(16) . . . 1_655 ?
O13 Mo1 O15 K3 94.24(14) . . . 2_556 ?
O14 Mo1 O13 K1 6.0(3) . . . 1_545 ?
O14 Mo1 O13 K3 125.33(12) . . . 1_655 ?
O14 Mo1 O15 K3 -130.00(14) . . . 1_655 ?
O14 Mo1 O15 K3 -22.63(15) . . . 2_556 ?
O15 Mo1 O13 K1 -107.8(3) . . . 1_545 ?
O15 Mo1 O13 K3 11.60(14) . . . 1_655 ?
O15 Mo1 O14 K3 162.2(2) . . . . ?
O15 Mo1 O14 K3 27.12(18) . . . 2_556 ?
O16 Al2 O10 K3 -101.98(11) . . . 2_566 ?
O16 Al2 O10 B6 114.8(4) . . . . ?
O16 B7 O17 K1 -16.0(3) . . . 2_576 ?
O16 B7 O17 B8 -174.3(3) . . . . ?
O16 B7 O18 K2 27.3(4) . . . 2_666 ?
O16 B7 O18 B9 -165.5(3) . . . . ?
O17 B7 O16 K1 16.0(3) . . . 2_576 ?
O17 B7 O16 K1 -68.6(3) . . . 1_554 ?
O17 B7 O16 Al2 152.6(2) . . . . ?
O17 B7 O18 K2 -152.52(18) . . . 2_666 ?
O17 B7 O18 B9 14.7(4) . . . . ?
O17 B8 O20 K2 164.1(2) . . . 2_566 ?
O17 B8 O20 K2 -117.2(2) . . . 1_454 ?
O17 B8 O20 B9 2.0(4) . . . . ?
O17 B8 O21 K2 -162.5(2) . . . 2_566 ?
O17 B8 O21 Al2 -20.0(5) . . . 1_455 ?
O18 B7 O16 K1 111.6(3) . . . 1_554 ?
O18 B7 O16 K1 -163.8(2) . . . 2_576 ?
O18 B7 O16 Al2 -27.3(4) . . . . ?
O18 B7 O17 K1 163.8(2) . . . 2_576 ?
O18 B7 O17 B8 5.5(4) . . . . ?
O18 B9 O19 K2 -13.2(2) . . . 2_666 ?
O18 B9 O19 Al1 105.2(2) . . . 2_566 ?
O18 B9 O19 B9 -112.6(2) . . . 2_565 ?
O18 B9 O20 K2 148.5(2) . . . 1_454 ?
O18 B9 O20 K2 -130.4(2) . . . 2_566 ?
O18 B9 O20 B8 16.7(4) . . . . ?
O19 Al1 O3 K2 64.10(13) 2_566 . . . ?
O19 Al1 O3 B2 -135.6(3) 2_566 . . . ?
O19 Al1 O7 B4 169.4(7) 2_566 . . . ?
O19 B9 O18 K2 14.2(2) . . . 2_666 ?
O19 B9 O18 K2 -85.54(18) 2_565 . . 2_666 ?
O19 B9 O18 B7 103.4(3) 2_565 . . . ?
O19 B9 O18 B7 -156.9(2) . . . . ?
O19 B9 O19 K2 99.49(13) 2_565 . . 2_666 ?
O19 B9 O19 Al1 -142.16(19) 2_565 . . 2_566 ?
O19 B9 O19 B9 0.002(0) 2_565 . . 2_565 ?
O19 B9 O20 K2 20.85(19) 2_565 . . 1_454 ?
O19 B9 O20 K2 -79.9(2) . . . 1_454 ?
O19 B9 O20 K2 102.0(3) 2_565 . . 2_566 ?
O19 B9 O20 K2 1.2(4) . . . 2_566 ?
O19 B9 O20 B8 -110.9(3) 2_565 . . . ?
O19 B9 O20 B8 148.4(2) . . . . ?
O20 B8 O17 K1 -159.74(17) . . . 2_576 ?
O20 B8 O17 B7 -13.8(4) . . . . ?
O20 B8 O21 K2 19.2(3) . . . 2_566 ?
O20 B8 O21 Al2 161.7(2) . . . 1_455 ?
O20 B9 O18 K2 145.83(19) . . . 2_666 ?
O20 B9 O18 B7 -25.2(4) . . . . ?
O20 B9 O19 K2 -145.66(19) . . . 2_666 ?
O20 B9 O19 Al1 -27.3(3) . . . 2_566 ?
O20 B9 O19 B9 114.9(3) . . . 2_565 ?
O21 Al2 O10 K3 134.93(10) 1_655 . . 2_566 ?
O21 Al2 O10 B6 -8.3(4) 1_655 . . . ?
O21 Al2 O16 K1 -79.47(11) 1_655 . . 1_554 ?
O21 Al2 O16 K1 -179.54(9) 1_655 . . 2_576 ?
O21 Al2 O16 B7 53.8(3) 1_655 . . . ?
O21 B8 O17 K1 21.9(4) . . . 2_576 ?
O21 B8 O17 B7 167.8(3) . . . . ?
O21 B8 O20 K2 -17.5(3) . . . 2_566 ?
O21 B8 O20 K2 61.2(3) . . . 1_454 ?
O21 B8 O20 B9 -179.6(2) . . . . ?

_olex2_submission_special_instructions 'No special instructions were received'
